# lattice dynamics studies of negative thermal expansion due

Embed Size (px)

TRANSCRIPT

Lattice Dynamics Studies of Negative Thermal Expansion Due to Two
Low-temperature Lattice Instabilities.11-27-2018

Follow this and additional works at: https://opencommons.uconn.edu/dissertations

Recommended Citation HANDUNKANDA, SAHAN UDDIKA, "Lattice Dynamics Studies of Negative Thermal Expansion Due to Two Low-temperature Lattice Instabilities." (2018). Doctoral Dissertations. 2021. https://opencommons.uconn.edu/dissertations/2021

Low-temperature Lattice Instabilities

ABSTRACT

Here I present a complete study of lattice dynamics of negative thermal ex-

pansion (NTE) material Scandium trifluoride (ScF3) and discovery of NTE in

mercurous iodide (Hg2I2). An inelastic x-ray scattering (IXS) study of ScF3

reveals copious evidence of an incipient soft-mode instability indicating that

the T=0 state of ScF3 is very close to a structural quantum phase transition

(SQPT). Is the anomalously strong and thermally persistent NTE behavior of

ScF3 a consequence of the SQPT? In order to address that, we have explored

the coefficient of thermal expansion (CTE) and soft mode behavior of a sec-

ond stoichiometric compound, situated near a SQPT. A detailed side-by-side

comparison of the metal trifluorides and mercurous halides suggest strong

similarities and a generic connection between the fluctuating ground state

of incipient ferroelastic materials and SNTE. We find experimental evidences

Sahan Handunkanda - University of Connecticut - 2018

for two- dimensional nanoscale correlations exist at momentum-space regions

associated with possibly rigid rotations of the perovskite octahedra of ScF3.

The discussion is extended by addressing the extent to which rigid octahedral

motion describes the dynamical fluctuations behind NTE by generalizing a

simple model supporting a single floppy mode that is often used to heuris-

tically describe instances of NTE. Temperature-dependent infrared reflection

measurement on single crystal ScF3 is performed to understand the zone cen-

ter lattice dynamics of ScF3. In addition, I also carried out an instrumentation

development project in the laboratory at the Department of Physics which will

be briefly discussed in the last chapter.

Lattice Dynamics Studies of Negative Thermal Expansion Due to Two

Low-temperature Lattice Instabilities

M.S. Physics, University of Connecticut, Storrs, CT, 2014 B.S. Physics, University of Colombo, Sri Lanka, 2009

A Dissertation Submitted in Partial Fulfillment of the

Requirements for the Degree of Doctor of Philosophy

at the University of Connecticut

2018

Lattice Dynamics Studies of Negative Thermal Expansion Due to Two

Low-temperature Lattice Instabilities

Major Advisor Jason Hancock

Associate Advisor Barrett Wells

Associate Advisor Douglas Hamilton

University of Connecticut 2018

iii

ACKNOWLEDGEMENTS

This thesis would not have been possible without collective effort and co- operation of many people. First of all, I would like to express my deepest appreciation to my PhD advisor Dr. Jason Hancock. I am greatly thankful for the faith that my advisor had on me from the day we first met, especially by welcoming me as his first graduate student. Throughout my PhD, I enjoyed and learnt from his knowledge and expertise in condensed matter research. He has given enormous encouragement and assistance while being patience with me over the past six and half years, something I truly appreciate. His characteristic traits eventually helped me to develop as a skilled physicist.

I also offer my sincere gratitude to Dr. Barrett Wells and Dr. Douglas Hamilton who served me as associate advisors. Apart from Dr. Wells’s proficiency and valuable discussion on my research I am also thankful to Dr. Wells for recom- mending me to talk with at the time new faculty member, Dr. Hancock about prospective research opportunities. I would like to thank Dr. Hamilton for his advise and encouraging words on writing which is the key to a successful scientific career.

I would like to express my gratitude to the beamline scientist Dr. Ayman Said at sector 30, Advanced Photon Source, Argonne National Laboratory for supporting us while we were taking our data on Scandium trifluoride samples. He provided a great amount of technical support during multiple beamtimes, which I never forget and greatly appreciate.

Successful experimentation is never possible without having quality samples. My special thanks goes to Dr. Vladimir Voronov in Kirensky Institute of Physics in Russia for proving us isotopically pure, single-crystalline Scandium triflu- oride samples and Dr. Sudhir Trivedi in Brimrose Technology Corporation, Sparks, Maryland for proving us single crystalline Mercurous Halide samples.

Theoretical collaborates are a vital part of a research study. The discussion we had and their insight on interpreting the experimentation results helped us to communicate and efficiently present the research findings and I would take this opportunity to thank the team led by Dr. Peter Littlewood then director of Argonne National Laboratory, Dr. Gian Guzman-Verri, and Dr.Richard Brier- ley in Yale University.

My sincere thanks goes to Dr. Joseph Budnick, Dr. William Hines, Dr. Boris

iv

Sinkovic, Dr. Gerald Dunne and Dr. Gayanath Fernando for the valuable con- versations that we had on our experimentation results. I appreciate Dr. Ilya Sochnikov and Dr. Diego Valente for accepting the invitation to take a part in my dissertation committee on such short notice. I would also like to thank to Dr. Dave Perry, someone who is always willing to help, especially when I need to figure out mechanical part necessary for my research work. Special thanks goes to Alan Chasse, the machine shop engineer for making all the necessary mechanical parts used in instrumentation development. I would also like to thank the former office staff Dawn, Kim and Babara as well as the current office staff in Physics, Micki, Anna, Caroline and Alessandra for their support in administrative works.

I would like to thank all my group members Erin Curry, Donal Sheets and Connor Occhialini whom I had a great time working with and had a lot of fun during my PhD in and out of the laboratory. The support and encouragement provided by Sri Lankan community at UConn, my batch mates Niraj, Zhiwei, Udaya, Susini, Katya and Dale at the difficult time during my stay at Storrs are hugely appreciated.

Last but not least I thank my dear parents, sister and my beloved wife Awanthi for their endless support and love provided me during the past few years.

v

TABLE OF CONTENTS

Ch. 1 : Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 1.1. Thermal expansion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 1.2. Lattice Dynamics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 1.3. Negative thermal expansion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9 1.3.1. Negative thermal expansion from phase competition . . . . . . . . . . . . . 10 1.3.2. Negative thermal expansion from framework dynamics . . . . . . . . . . 13 1.4. Theoretical consideration of negative thermal expansion . . . . . . . . . . . 16 1.4.1. Grneisen theory and thermal expansion . . . . . . . . . . . . . . . . . . . . . . . . . 16 1.4.2. Rigid unit mode picture . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 17 1.4.3. Tension effect and NTE . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 21 1.4.4. Thermodynamics of NTE materials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 21 1.5. Perovskites . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 22 1.6. Trifluorides and their structures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 23 1.7. Scandium trifluoride(ScF3) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 25 1.7.1. Negative thermal expansion in ScF3 . . . . . . . . . . . . . . . . . . . . . . . . . . . . 25 1.7.2. Pressure induced phase transition in ScF3 . . . . . . . . . . . . . . . . . . . . . . . 26 1.7.3. Electronic structure of ScF3 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 27 1.8. Motivation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 29

Ch. 2 : Lattice dynamics study of ScF3 using inelastic x-ray scattering . . . 31 2.1. Introduction to Inelastic X-ray Scattering . . . . . . . . . . . . . . . . . . . . . . . . . . 31 2.1.1. IXS advantages over other spectroscopic techniques . . . . . . . . . . . . . . 32 2.2. Scattering theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 34 2.2.1. Dynamic structure factor (S(

−→ Q, ω)) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 39

2.2.2. Quantum mechanical perspective . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 41 2.2.3. Scattering cross section . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 48 2.2.4. IXS for phonons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 49 2.2.5. Scattering from phonons in theoretical perspective . . . . . . . . . . . . . . 51 2.3. Inelastic X-ray Scattering on ScF3 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 55 2.3.1. The Experiment . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 56 2.3.2. Single crystal ScF3 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 56 2.3.3. Lattice parameter measurement . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 61 2.3.4. Phonon dispersion relation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 62 2.3.5. M-R branch and NTE . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 63 2.3.6. M-R branch and phase transition . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 64 2.3.7. Central peak of ScF3 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 67 2.3.8. What causes central peak? . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 68 2.3.9. Central peak of ScF3 and mode softening . . . . . . . . . . . . . . . . . . . . . . . . 72

vi

2.3.10. Quantum phase transition in ScF3 and phase transitions in other transition metal trifluorides . . . . . . . . . . . . . . . . . . . . . . . . . . . . 76

2.3.11. ScF3 systems and disorder . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 78 2.3.12. Transverse motion of F atoms . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 81 2.3.13. Elastic parameters of ScF3 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 82 2.3.14. Modeling IXS data using Damped Harmonic Oscillator(DHO) . . . . 86

Ch. 3 : Comparative study of two incipient ferroelastics, ScF3 and Hg2I2 92 3.1. Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 92 3.2. Low-T structure and scattering evidence for the IFE behavior of

Hg2I2 and ScF3 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 94 3.3. Discussion and SNTE material design principles . . . . . . . . . . . . . . . . . . . 98

Ch. 4 : Thermal Diffuse Scattering on ScF3 . . . . . . . . . . . . . . . . . . . . . . . . . . . 106 4.1. Introduction to diffuse scattering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 106 4.2. Diffuse Scattering study of single-crystalline compound ScF3 . . . . . . . 107 4.2.1. Experiment . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 107 4.2.2. Negative thermal expansion of ScF3 and diffuce scattering . . . . . . . 108 4.2.3. Results and discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 110

Ch. 5 : Two dimensional constrained lattice model to study ScF3 lattice . 114 5.1. Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 114 5.2. Two-dimensional constrained lattice model . . . . . . . . . . . . . . . . . . . . . . . 115 5.3. Application of model to experimental results . . . . . . . . . . . . . . . . . . . . . . 121

Ch. 6 : Infrared study of ScF3 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 125 6.1. Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 125 6.2. Measurements . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 126 6.3. Lorentzian model fitting . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 127 6.4. Factorized model fitting . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 128 6.5. Zone center modes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 132 6.6. Infrared measurement results . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 134 6.6.1. Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 137

Ch. 7 : Resonant Ultrasound Spectroscopy . . . . . . . . . . . . . . . . . . . . . . . . . . . . 147 7.1. Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 147 7.2. Elastic properties and constitute equations . . . . . . . . . . . . . . . . . . . . . . . . 148 7.2.1. Symmetries in cubic systems and other important properties . . . . . . 151 7.3. Resonant ultrasound spectroscopy fundamentals . . . . . . . . . . . . . . . . . . 154 7.4. ScF3 sample and RUS setup used . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 156 7.5. RUS measurement on ScF3 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 158

Ch. 8 : Instrumentation Development . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 164 8.1. Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 164

vii

App. A : Construction of an optical system . . . . . . . . . . . . . . . . . . . . . . . . . . . 186

Bibliography . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

viii

LIST OF FIGURES

1.1.1 (a) The anharmonic potential is shown. The potential is asym- metric, so that increases in temperature (i.e. the amplitude of oscillation of atoms) leads to an increase in the mean interatomic separation, and hence to thermal expansion. (b) The harmonic potential is symmetric and as the temperature is increased the mean separation remains the same hence no thermal expansion . 3

1.2.1 A linear chain of identical atoms. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 1.2.2 Dispersion relation of the 1D chain of atoms. . . . . . . . . . . . . . . . . . . . . 6 1.2.3 A linear chain of two atomic species . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7 1.2.4 Dispersion relation of the 1D chain of two different atoms. . . . . . . . . 9 1.3.1 NTE in ferroelectrics. (a) Unit cell volume of 0.5PbTiO3-0.5(Bi1−xLax)FeO3

(x = 0.0, 0.1, and 0.2) as function of temperature. FE and PE mean ferroelectric and paraelectric, respectively. Taken from [1]. (b) Thermal expansion coefficient of volume in PbTiO3.Taken from [2]. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11

1.3.2 NTE due to valance transitions. (a)Temperature dependence of the unit cell volume of BiNiO3. Low pressure-temperature and high pressure-temperature data are drawn as open and closed circles, and crosses show the weighted average volume in the transition region. From [3]. (b)The dilatometric linear thermal expansion of Bi0.95La0.05NiO3 on heating and cooling showing a 20 K hysteresis. From [3]. (c)Temperature evolution of structure parameter unit cell volume of Sm2.75C60.From[4] . . . . . . . . . . . . . . . 12

1.3.3 NTE in magnetic materials. (a) Temperature dependence of the unit-cell volume of MnF3 . The Neel temperature, TN is shown. From [5]. (b) Relative length changes L/L0 of ferromagnet GdAgMg for various magnetic fields. From [6] . . . . . . . . . . . . . . . . 14

1.3.4 Negative thermal expansion in ZWO. Filled circles represent neu- tron diffraction data while open circle represent dilatometry data. Taken from [7]. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 15

1.4.1 Rotation of 2D perovskite leads to an area reduction. . . . . . . . . . . . . . 20 1.4.2 Representation of the tension effect. A linear linkage of three atoms

is shown in left. This can distort such a way that the central atom displaces transverse direction or the two end atoms displace in opposite ways. In both cases the bonds stay in rigid and the two end atoms move inwards in the vertical direction. Taken from [8] 22

1.6.1 Global structural phase diagram of MF3 type perovskites. . . . . . . . . . 24

ix

1.7.1 Pressure-temperature phase diagram for ScF3. The dashed line is a guide to the eye. Two layers of octahedra in both the cubic and the rhombohedral ReO3 structures (viewed along [111]) are shown. Upon pressurization, octahedral tilts fold the structure so that it is more compact and reduce the symmetry from cubic to rhombohedral. Taken form [9] . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 28

2.1.1 Excitations that may probe using IXS, From [10] . . . . . . . . . . . . . . . . . . 31

2.2.1 X-ray scattering from an arbitrary atoms . . . . . . . . . . . . . . . . . . . . . . . . . 34

2.2.2 Radiation from source (S) to detector (D) via the sample . . . . . . . . . . . 37

2.2.3 Reflection geometry where the blue solid circle represents the jth

atom where −→r j and −→r initiate at the unit cell origin . . . . . . . . . . . . . . 38

2.2.4 Typical features appear on high energy resolution inelastic scatter- ing spectrum . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 50

2.2.5 Phonon creation is shown on left and phonon annihilate process on right . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 51

2.3.1 Simple cubic structure of ScF3 lattice where pink spheres are Sc atoms and orange spheres represent F atoms. From [11] . . . . . . . . . 57

2.3.2 Schematic of IXS spectrometer layout (a) and photograph (b) of the 9 m arm of the spectrometer at sector 30 of APS. The schematic is not to scale. The main components, the direction of incident beam and scattered beam are shown. Sample is mounted on a four circle rotational mount and the detector array is kept as much as close to the sample. Analyzer array is mounted at far end of the arm which is capable of rotate about 32 degrees which is corresponding to maximum of 75 nm−1 momentum transfer. . . . 57

2.3.3 (a) Single crystal ScF3 received from Vladimir Voronov. We named them for identification purpose in future usage. (b) Simple cubic structure formation of ScF3 lattice drawn in to scale where purple spheres are Sc atoms and red spheres represent F atoms. . . . . . . . . 58

2.3.4 (a) Crystal mount used in sector 30 experiment. (b) Dimensions of the crystal Gamma. Crystal sits on wax in order to carry out X-ray diffraction measurement. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 59

2.3.5 Diffraction spots appeared on 2D area detector. Crystal plane is z=o and sample Gamma is used. Lattice planes are shown in dotted lines . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 60

2.3.6 X -ray diffraction data on powder ScF3 sample . . . . . . . . . . . . . . . . . . . 60

x

2.3.7 (a) Mosaic width ∼ 0.0020, as measured on the strong (H,K,L) = (1,1,0) Bragg reflection indexed to the four-atom simple cubic cell (lattice parameter a = 4.016 A at temperature T = 300 K) (b) Lattice volume as a function of temperature determined from tracking the Bragg peak (3,0,0) in single-crystalline ScF3. Inset: The lattice volume over a larger thermal window determined on powder samples[9]. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 61

2.3.8 Overview of the lattice mode dispersion at select momenta and energies. Strong branch softening along the M − R cut is shown by arrows. The longitudinal (LA) and transverse (TA) acoustic branches are shown. Black solid lines are a guide to the eye. Red circles in the inset mark the momenta R + δ (2.39,1.43,0.45) and M + ε (2.39,1.43,0.02) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 62

2.3.9 100 planar section of the octahedra, illustrating the displacement pattern of modes attributed to NTE. The area of the box in (b) is reduced by cos2θ of the area in (a) . . . . . . . . . . . . . . . . . . . . . . . . . . . . 64

2.3.10 First Brillouin zone of simple cubic material ScF3. High symmetry points are shown as well. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 65

2.3.11 (a) The lowest vibrational modes at the M point.(M+ 3 distortion) (b)

The lowest vibrational modes at the R point. The rhombohedral phase can be described as a static tilt according to the R+

4 pattern. 66 2.3.12 (a) Inelastic spectra of SrTiO3 measured at several temperatures.

Left side shows the soft mode behavior and right side shows divergence of central peak. From [12]. (b) Inelastic spectra of SrTiO3 (left) and KMnF3 (right) for approximately equal T=T- Tc. From [12]. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 68

2.3.13 Central peak due to defects and impurities. (a) Integrated central peak intensity of hydrogen reduced SrTiO3 as a funtion of T-Tc [13]. (b) The temperature dependence of the central peak height of the as-grown KH3(SeO3)2 crystal (+) and the crystals used repeatedly (0, ,x)[14] . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 70

2.3.14 Broad and narrow features within the central peak. Solid and dotted curves in (a) represent fitting models, Lorenzian squared

and Lorenzian function respectively[15]. (b) X-ray scans of 1 2

(1,1,5) R point along [0 1 1] direction with 100 keV photon energy beam hitting at the center of the crystal and (c) beam hitting the crystal corner of the crystal. )[16] . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 71

2.3.15 Color maps of the IXS signal at the (a) M (b) R points in reciprocal space . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 73

2.3.16 Color maps of the IXS signal at the (c) M +ε, and (d) R + δ points in reciprocal space. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 73

xi

2.3.17 Resolution convoluted fitting of the IXS data in figure 2.3.16 results in squared mode energies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 74

2.3.18 Resolution convoluted fitting of the IXS data in figure 2.3.16 results in elastic peak intensity. Elastic peak begins to appear near 80 K, which is 120 K above the extrapolated transition temperature. . . . 75

2.3.19 Central peak intensity observed in SrTiO3 [17]. Elastic peak begins to appear 25 K above the transition and the intensity reaches it’s maximum at the transition temperature. . . . . . . . . . . . . . . . . . . . . . . . 75

2.3.20 Cubic and rhombahedral unit cells associated with two phases of transition metal trifluorides other than ScF3 are shown. As shown the rhombahedral phase is associated with rotated ScF6

sub units. Gray circles represent scandium atoms and light blue circles represent fluorine atoms. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 77

2.3.21 Structural phase diagram showing the c-r phase boundary vs the B-site mean radius in 3d transition metal trifluorides and in the solid solutions Sc1xAlxF3 and Sc1xYxF3. Data taken from Refs [18, 19, 20, 21, 22]. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 79

2.3.22 Disorder phase diagram for ScF3. Compositional disorder is quan- tified via the B-site variance σ2

B = rB - rB 2, which has the effect

of increasing the stability of the lowersymmetry, rhombohedral structural phase. Red and orange symbols show the effect of Y and Al substitution, respectively. Dotted lines indicate a linear fit to the Tc(σ2

B), not including the pure sample ScF3. The verti- cal axis intercept reveals a temperature scale ∼ 80-100 K,where central peak elastic scattering and thermal expansion saturation are also observed in pure ScF3 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 81

2.3.23 Transverse vibrations of Fluorine atom . . . . . . . . . . . . . . . . . . . . . . . . . . 82 2.3.24 Acoustic phonon energies along different directions in reciprocal

space. The slope simply gives the acoustic velocities of corre- sponding modes along different directions for ScF3. LA and TA stands for longitudinal acoustics and transverse acoustics respectively . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 83

2.3.25 Poisson ratio obtained from elastic parameters . . . . . . . . . . . . . . . . . . . 85 2.3.26 Youngs modulus obtained using elastic parameters . . . . . . . . . . . . . . . 86 2.3.27 Representative resolution function collected at 6K from plexiglass

co-mounted with the sample . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 88 2.3.28 Schematic of the dynamical structure factor used to fit the data . . . . 89 2.3.29 Sample of fit quality at momentum points R (left column) and M

(right column). The red points and blue lines resemble data and the fit respectively. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 90

2.3.30 Sample of fit quality at momentum points R+δ (left column) and M + ε (right column). . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 91

xii

3.2.1 Structural phase diagrams of (a) 3d transition metal trifluorides and (b) mercurous halides. Insets show the basic volume-defining polyhedral units: (a) the BF6 octahedraon and (b) the elongated square dipyramid (ESD). Development of the structure for (c) the trifluorides and (d) the mercurous halides with the ionic radii indicated as spheres. The basic polyhedral structural unit is superposed in each case. (e) Comparison of the observed bond distances (symbols) and expectations based on hard sphere packing (dashed lines). . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 95

3.2.2 Temperature-dependent lattice parameters of (a,c) ScF3, TiF3, and (b,d,f) Hg2I2, and Hg2Br2. (e) shows a schematic free energy landscape of realized and incipient ferroelastics. Arrows show the fluctuation domain in each case. . . . . . . . . . . . . . . . . . . . . . . . . . . . 96

3.2.3 Rocking curves measured at (330) bragg peak for optical and detec- tor quality Hg2Br2 and Hg2I2 crystals cleaved along 110 planes grown by physical vapor deposition method by Brimrose Tech- nology Cooperation. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 97

3.3.1 Structure of 3d transition metal trifluorides in the (a) high-temperature cubic phase and (b) the low-temperature rhombohedral phase. Structure of the mercurous halides in (c) the high-temperature body-centered tetragonal and (d) low-temperature orthorhom- bic phases. Inelastic X-rays scattering measurement of (e) ScF3

at the simple-cubic R point, corresponding to the soft mode of the rhombohedral transition and (f) Hg2I2 at the BCT X point, corresponding to the soft mode of the orthorhombic transition. Insets show the Brillouin zone in each case. Soft mode frequency squared resultant from fitting to a damped-harmonic oscillator model for (g) ScF3 at R point and (h) Hg2I2 at X point. Dashed lines indicate the extrapolation to negative absolute temperature and indicate the proximity to an incipient ferroelastic transition. . 100

3.3.2 Structure of 3d transition metal trifluorides in the (a) high-temperature cubic phase and (b) the low-temperature rhombohedral phase. Structure of the mercurous halides in (c) the high-temperature body-centered tetragonal and (d) low-temperature orthorhom- bic phases. Inelastic X-rays scattering measurement of (e) ScF3

at the simple-cubic R point, corresponding to the soft mode of the rhombohedral transition and (f) Hg2I2 at the BCT X point, corresponding to the soft mode of the orthorhombic transition. Insets show the Brillouin zone in each case. Soft mode frequency squared resultant from fitting to a damped-harmonic oscillator model for (g) ScF3 at R point and (h) Hg2I2 at X point. Dashed lines indicate the extrapolation to negative absolute temperature and indicate the proximity to an incipient ferroelastic transition. . 103

xiii

4.2.1 Thermal diffuse scattering images of (a) (100) (b) (110) (c) (111) planes taken for ScF3. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 110

4.2.2 Inset: Experimental geometry for the diffuse scattering experi- ments in single-crystal ScF3. Main panel shows a H = 0.5 cross section of the Ewald sphere. Blue and orange arcs indicate the extrema of the crystal rocking angle(1 ) . . . . . . . . . . . . . . . . . . . . . . . 112

4.2.3 (a) Diffuse scattering intensity collected using the experimental geometry in Figure 4.2.2. Mid-zone intensity at M points are indicated by dashed circles and are found in almost every BZ. Dashed lines indicate cuts through the intensity patterns shown in (b). Each cut in (a) is taken an an equivalent K value but corresponds to a different L value. The negligible change in widths is strong evidence of 2D spatial correlations. . . . . . . . . . . . . 113

5.1.1 (a) A 5 × 5 × 5 crystallite of ScF3 in the average structure (125 octahedra). (b) The hollow cube shows the simple cubic BZ with shaded regions indicating the positions of observed scattering rods from the data in Figure 4.2.3. Breakouts show possible real- space staggered rotation patterns which preserve internal octa- hedral dimensions at the indicated high-symmetry momentum- space points. Red and blue shading in the diamonds indicate equal but opposite magnitudes of rotation. . . . . . . . . . . . . . . . . . . . . . 115

5.1.2 A model consisting of stiff diamonds connected by hinged joints shown. As a result of the constraints, a staggered rotation by an angle θ in (b) causes a shortening of the vector locating each diamond by a factor cos θ . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 116

5.2.1 (a)(d) show classical solutions for θ(t) which follow from Equation 5.2.3. These are plotted for different values of k0, which uniquely quantifies the anharmonic behavior. The time axes in (a) and (c) are scaled by the FM period . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 120

5.3.1 (a) Lattice parameter of ScF3 below T = 300 K from Ref. [23] (b) Transverse fluorine thermal parameter determined from x- ray pair density function analysis [18]. Superimposed on (a) and (b) are the corresponding quantities from (2) using Nx = 5.5 for varying values of ~ωp (c) Velocity field superimposed on a homogeneously excited FM, with phase and kinetic energy below. (d) shows the significant kinetic energy lowering when a π/2 defect is introduced. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 123

6.4.1 A sample spectra taken for ScF3. The frequency-dependent optical behavior of ScF3 is divided in regions: T for transmission (or ”transparency”), A for absorption and R for reflection. . . . . . . . . . . 132

xiv

6.4.2 Compare the parameters obtained from factorized form model and Lorentzian model. Black markers are obtained from lorentzian model and colored plots are from factorized form model. . . . . . . . . 133

6.5.1 Gray sphere represents Sc atom while Blue spheres represent F atoms. Black arrows show the direction of displacement. (a) Acoustic mode. (b) The lowest energy optical mode. This is also known as silent mode (c) The highest energy mode (TO2 in our case) (d) The low energy mode which is also known as breathing mode.(TO1 in our case) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 134

6.6.1 Measured reflectance of ScF3 sample at different temperatures . . . . . 135 6.6.2 (a),(c) TO phonon energies & (b),(d) LO phonon energies obtained

for ScF3 by fitting the reflection with factorized formula at dif- ferent temperatures. Corresponding linewidths obtained are shown in insets . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 138

6.6.3 (a) Temperature dependance of imaginary part of permitivity ,Imε(ω). Peak values are corresponding to TO phonon peaks. The inset shows the resulted peak due to two phonon scattering. The In- set scale is magnified by 100. (b) Temperature dependance of loss function,-1/Imε(ω). Peak values are corresponding to LO phonon peaks. The inset shows the resulted peak due to two phonon scattering. Inset scale is magnified by 100 . . . . . . . . . . . . . . 139

6.6.4 Variation of the real part of the dielectric function for ScF3 with temperature. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 140

6.6.5 Most probable combination of two phonons are shown. They could be arising from sharp DOS which is shown in extended blue area in combined plots of phonon dispersion and corre- sponding DOS. Directions along Γ - M - R and along Γ - X - M are considered. A mode lies at momentum point -q with in red( at momentum point q in green) areas of dispersion plot corresponding to higher energy DOS peak and a mode lies at momentum point q with in red( at momentum point -q in green) areas in the lower energy DOS peak excite and correspond to two phonon absorption. Dispersion plots are taken from [24] . . . . 145

7.2.1 Stress tensor components acting on a body with respect to a three- dimensional Cartesian coordinate system . . . . . . . . . . . . . . . . . . . . . 151

7.2.2 Information hidden in elastic stiffness tensor elements are shown in matrix form for clear view . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 152

7.3.1 Typical setup used for RUS measurements . . . . . . . . . . . . . . . . . . . . . . . 155 7.4.1 (a) Single crystal ScF3 used for RUS measurement. This is the

second shipment of crystal received from Vladimir Voronov. (b) Experimental setup used in Los Alamos National Laboratory . . . . 157

xv

7.5.1 Typical example of RUS signal. Two sharp peaks indicate reso- nance vibrations of ScF3 lattice around 500 kHz . . . . . . . . . . . . . . . . 159

7.5.2 Resonance vibrations around 600 kHz . . . . . . . . . . . . . . . . . . . . . . . . . . . 159 7.5.3 Temperature dependence resonance(around 775 kHz) for crystal

ScF3. Red line indicates the energy dissipation or the width of the resonance peak as a function of temperature . . . . . . . . . . . . . . . . 161

7.5.4 Temperature dependence resonance(around 380 kHz) for crystal ScF3. Red line indicates the energy dissipation or the width of the resonance peak as a function of temperature . . . . . . . . . . . . . . . . 162

8.2.1 Spherical mirror wouldn’t be the best choice when the object and the image is non collinear . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 167

8.2.2 Prolate ellipsoid with two planes of interests. Two planes are orthoganal to each other. Unit vector represents the center of the to be constructed mirror. Two orthogonal ROCs are given by the projections of the planes on the ellipsoids . . . . . . . . . . . . . . . . . . . . . . 169

8.2.3 Prolate ellipsoid with focii at(−d, 0, 0) and (d, 0, 0). (x0, 0, z0) denotes the center position of the to be constructed mirror with specifica- tions s, t and α. They denote the object distance, image distance and the angle in between respectively. . . . . . . . . . . . . . . . . . . . . . . . . . 170

8.2.4 Exact surface in which the mirror is grinded is the ellipsoidal shape shown in green. But in our design process we used toroidal surface shown in red as an approximations to the ellipsoidal shape. The point of interest in which the two orthogonal ROC were calculated is (x0, 0, z0). Orange bordering around the point of interest approximately represents the mirror surface obtained. . 171

8.2.5 Optical layout combined with cryocooler. Specifications of each mirrors are given in Table 6.1. Gray colored mirrors are plane mirrors and the whole layout can be rotated around them. A sharp aperture is placed at the focus of M0 mirror. This defines the object to M1 mirror which forms an image at the sample space. Light reflects from and transmits through the sample are collected by M2r and M2t mirrors and refocused into detec- tors(Red colored) by M3r and M3t mirrors . . . . . . . . . . . . . . . . . . . . . . 172

8.2.6 Custom made components for optical cryocooler. . . . . . . . . . . . . . . . . 174 8.3.1 THz frequency range with respect to the whole electromagntic

spectrum. The range approximately is in between 2 meV and 20 meV. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 176

8.3.2 Current THz spectrometer. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 179 8.3.3 Comparison between electro-optic detection and antenna detection

setups . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 180 8.3.4 The virtual source point for the BATOP antenna is roughly = L - d

= 18.7 mm behind the antenna chip . . . . . . . . . . . . . . . . . . . . . . . . . . . 182

xvi

8.3.5 Time Domain THz signal . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 185 8.3.6 Frequency Domain THz signal . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 185

A.3.7 ellipse shown in xyz coordinate,y is perpendicular to the plane . . . . 186 A.3.8 two coordinate systems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 190 A.3.9 ellipse representing in two coordinates . . . . . . . . . . . . . . . . . . . . . . . . . . 191

xvii

LIST OF TABLES

2.1.1 List of techniques broadly grouped under the heading of Inelastic X-Ray Scattering.From[10] . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 32

2.3.2 Summary of elastic properties of similar type of materials. Bulk modulus (B), Shear modulus (G) and Zener anisotropy (A) are shown as well . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 84

6.6.3 Compare the fit models at 300 K. Unites are given in cm−1 . . . . . . . . . 136 6.6.4 Comparison of our experimental results with previous calculations

at 300 K. Units of energies are cm−1. . . . . . . . . . . . . . . . . . . . . . . . . . . . 137 6.6.5 Static dielectric constant for ScF3 obtained from LST relation . . . . . . . 143 6.6.6 Two phonon absorption possibilities, if only high symmetric points

are considered . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 144

8.2.7 Specifications of mirrors used in mirror layout shown in Figure 8.2.5. Here∞means the beam is parallel. The mirror notation is used for identification purpose. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 173

xviii

1.1 Thermal expansion

Materials tendency to decrease or increase their volume when heated is known

as thermal expansion. The vast majority of materials increase in dimension

when they are heated corresponding to positive thermal expansion (PTE).

While thermal expansion is common among all three phases of substances, in

solids it may be isotropic or anisotropic. Substances expand in same amounts

along any direction known as isotropic expansion, which is different from

anisotropic case where materials expand in different amounts along different

crystallographic orientations.

Thermal expansion in solids is a direct consequence of the anharmonic nature

of interatomic forces between atoms (anharmonic potential) (Figure 1.1.1a).

The mean separation between atoms correspond to the minimum potential is

identified as the equilibrium distance between them. As the temperature is

increased the potential energy of the system increases and the asymmetry of

potential suggests an increase in mean separation, hence thermal expansion.

On the other hand if the atoms behave in harmonic manner, then the mean

1

separation between atoms would not change even the vibrational amplitude

increases with increasing temperature, hence no thermal expansion (Figure

1.1.1b).

Thermal expansion is typically quantified by using coefficient of thermal expan-

sion(CTE), which simply is the relative change in material dimension within

a given change in temperature at constant pressure. In order to measure

the relative change along a certain directions in a solid object, the linear

CTE, αL = (1/L)(∂L/(∂T)P, is defined and this is frequently used to quantify

anisotropic thermal expansion. The magnitude of the thermal expansion is

mostly expressed in terms of volumeteric CTE, αV = (1/V)(∂V/(∂T)P where V is

volume, T is temperature and P is pressure. The CTEs is expressed in unit K−1

and for solids in general the CTEs are of the order of 10−6 and the unit ppm/K

is used instead.

1.2 Lattice Dynamics

Lattice dynamics is the study of vibrations of the atoms in a crystal. It is an

important phenomenon to understand and governs the key properties of mate-

rials such as thermodynamics, phase transition, thermal conductivity, thermal

expansion, and sound wave propagation. More importantly it interacts with

electromagnetic radiation. In lattice dynamics study the atomic motions are

described by traveling waves. Each wave is characterized by wavelength λ,

angular frequency ω, amplitude and direction of travel. For the convenience

2

Figure 1.1.1: (a) The anharmonic potential is shown. The potential is asymmet- ric, so that increases in temperature (i.e. the amplitude of oscillation of atoms) leads to an increase in the mean interatomic separation, and hence to thermal expansion. (b) The harmonic potential is symmetric and as the temperature is increased the mean separation remains the same hence no thermal expansion

wavelength is being replaced with wave vector k= 2π/λ.

Simplest form of lattice dynamics theory uses harmonic approximation. Con-

sidering the potential given in Figure 1.1.1a the Taylor series expansion around

equilibrium distance between atoms, r0 can be written as

V(r) = V0 + 1 2 ∂2V ∂r2 (r − r0)2 +

1 3! ∂3V ∂r3 (r − r0)3 +

1 4! ∂4V ∂r4 (r − r0)4 + .... (1.2.1)

In harmonic approximation only the quadratic terms is retained. In most cases,

the approximation is very effective and if not, we can start with it and then

modify the model by adding higher order terms for better results of inter-

3

atomic forces, wave vectors and frequencies. Nevertheless, properties such

as thermal conductivity, thermal expansion, and phase transition can not be

explained by the harmonic model.

Consider a crystal with one atom per unit cell, as an example, a 1D chain of

atom, each of mass m. The atoms are connected by elastic springs, so the force

between the atoms are directly proportional to relative displacement from the

equilibrium position. Let us assume that the separation between consecutive

atoms is a, so the position of the nth atom in 1D chain is na (Figure 1.2.1). We

define the displacement of nth atom to be Un and write equation of motion of

an atom

Fn = C((Un+1 −Un) − (Un −Un−1)) = m d2Un

dt2 (1.2.2)

where C is the force constant.

For any coupled system, a normal mode is defined to be a collective oscillation

where all particles move at the same frequency. Let us now attempt a solution

4

Un = U0ei(ωt−kna) (1.2.3)

where U0 is the amplitude of oscillation and k is the wave vector.

Plugging the solution to Equation 1.2.2 we get

−mω2U0ei(ωt−kna) = CU0eiωt[e−ika(n+1) + e−ika(n−1) − 2e−ikan] (1.2.4)

mω2 = 2C[1 − cos(ka)] = 4C sin2(ka/2) (1.2.5)

and we obtain the result

ω = 2

√ C m

sin (ka

2

). (1.2.6)

The relationship, ω(k) is known as the dispersion relationship of the correspond-

ing atomic structure. Figure 1.2.1 shows the dispersion relation and it is pe-

riodic in k → k + 2π/a. Following this we use the term k-space which is also

known as reciprocal space. The periodic unit in reciprocal space is known as Bril-

louin Zone(BZ) and Figure 1.2.1 shows only the ”First Brillouin Zone” which

has the boundaries at k= ±π/a.

5

Figure 1.2.2: Dispersion relation of the 1D chain of atoms.

One important consequence of dispersion relationship in 1D chain is that it

allows us to calculate group velocity, Vg = dω/dk and phase velocity, Vp =

ω/k. With the particular dispersion relation given in Equation 1.2.6 the group

velocity

Vg = 2(Ca2/m)1/2 cos(ka/2). (1.2.7)

In long wavelength limit, where cos ka ∼ 1-(ka/2)2, the dispersion relation be-

comes

ω2 = (C/m)(k2a2) (1.2.8)

and we obtain a result that the velocity in long wave length limit is independent

6

of frequency. Recalling that the sound wave is a vibration that has long wave

lengths, we obtain the result

Vsound = a

√ C m . (1.2.9)

We discussed a classical system which has normal mode of frequency ω. The

corresponding quantum mechanical system will have eigenstates with energy

En = ~ω(n + 1 2

) (1.2.10)

which the energy of a lattice vibrations is quantized and quantum of energy

is called Phonon. This is analogues to quantized energy called photons of the

electromagnetic wave.

We now extend the discussion to analyze linear chain with two atomic species

(Figure 1.2.3). Writing down equations of motions

Figure 1.2.3: A linear chain of two atomic species

7

dt2 (1.2.11)

dt2 (1.2.12)

Un = U0ei(ωt−kna) (1.2.13)

Vn = V0ei(ωt−kna) (1.2.14)

(C1 + C2eika)U0 + (mω2 − C1 − C2)U0 = 0 (1.2.16)

where for simplicity here we used m1=m2.

The solutions to this are obtained by finding the zeros of secular determinant (mω2

− C1 − C2) (C1 + C2e−ika)

(C1 + C2eika) (mω2 − C1 − C2)

= 0

8

1 + C2 2 + 2C1C2 cos(ka). (1.2.17)

Figure 1.2.4: Dispersion relation of the 1D chain of two different atoms.

This method can be generalized for more complex three-dimensional materials

and most of the advanced condensed matter textbooks explain this approach

thoroughly. To complete the normal mode solution in three dimensional, the

vibrational amplitude should be incorporated which can be used to calculate

the total energy of the crystal as well.

1.3 Negative thermal expansion

It is not uncommon that some materials show the opposite behavior of PTE,

9

which they shrink upon heating give rise to negative thermal expansion (NTE).

This is relatively new filed of study, yet we have seen phenomenal development

in recent years as many materials are discovered displaying this unusual be-

havior. The most popular example for NTE phenomenon is the liquid water-ice

expansion below 40 C and above ice-water phase boundary.

Even though not all of the different mechanisms responsible for NTE are fully

understood, generally the origin of NTE is viewed in two different ways. NTE

could either arise from non-vibrational effect associated with electronic and

magnetic instabilities or emerge from vibrational effect associated with intrinsic

geometrical instabilities.

1.3.1 Negative thermal expansion from phase competition

The non-vibrational effects account for NTE are mostly related with phase

transitions and one of the very well known example for this type of materials

family is ferroelectrics. Interestingly, some ferroelectrics exhibit NTE or anoma-

lous thermal expansion properties below the curie temperatures and their NTE

originates from ferroelectric order which occurs due to the strong hybridization

between cations and anions. Some of the notable examples in this category are

PbTiO3[2, 25, 26, 27],PbTiO3 based compounds[28, 1], BaTiO3[29], BiFeO3[25],

Pb(Zn1/3Nb2/3)O3[30], Ca3Mn2O7[31], Ca3Ti2O7[31] and Sn2P2S6[32]. The NTE

associated with the spontaneous polarization originating from Pb/Bi-O hy-

bridization is reported for PbTiO3-based compounds [28] and they have at-

10

tracted attention due to the precise capability of controlling NTE, not just in

a single way but by using various methods such as the chemical modifica-

tion, size effect, and physically by applying pressure. A couple of examples of

ferroelectric NTE are shown in Figure 1.3.1.

Figure 1.3.1: NTE in ferroelectrics. (a) Unit cell volume of 0.5PbTiO3- 0.5(Bi1−xLax)FeO3 (x = 0.0, 0.1, and 0.2) as function of temperature. FE and PE mean ferroelectric and paraelectric, respectively. Taken from [1]. (b) Ther- mal expansion coefficient of volume in PbTiO3.Taken from [2].

The change of electron configuration can also cause NTE and abnormal thermal

expansion properties to some materials. The volume increment upon cooling

due to a valance transition has been reported for rare earth fulleride Sm2.75C60

[4]. NTE in BiNiO3 [3] is attributed to atomic radius contraction caused by

intermetallic charge transfer from Ni to Bi. Others display NTE due to intersite

charge transfer, as reported in perovskites oxides such as SrCu3Fe4O12[33] and

LaCu3Fe4O12[34]. Even semiconductors (e.g. Si, Ge, and GaAs [35, 36]), su-

perconductors (e.g. MgB2, Ba(Fe0.926Co0.074)2As2 [37, 38]) and Mott insulators

(e.g. Ca2RuO4 based compounds [39, 40] ) exhibit NTE or anomalous thermal

11

expansion properties as a result of change in electron configuration. There exist

a number of ways to tune NTE due to phase competition, including controlling

free electron concentration of semiconductors, modulating the metal insulator

transition of Mott insulator, and introducing quenched disorder. An attribute

of this approach is the potentially large CTE, although a drawback in most

cases is persistence over only a narrow temperature range.

Figure 1.3.2: NTE due to valance transitions. (a)Temperature dependence of the unit cell volume of BiNiO3. Low pressure-temperature and high pressure- temperature data are drawn as open and closed circles, and crosses show the weighted average volume in the transition region. From [3]. (b)The dilatomet- ric linear thermal expansion of Bi0.95La0.05NiO3 on heating and cooling showing a 20 K hysteresis. From [3]. (c)Temperature evolution of structure parameter unit cell volume of Sm2.75C60.From[4]

A change in volume in response to staggered or uniform spontaneous magneti-

12

zation is known as magnetovolume effect” has been identified as the cause for

anomalous thermal expansion of magnetic materials. The underlying nature

of NTE or anomalous thermal expansion in magnetic materials is the coupling

between magnetic order and the lattice. The first discovery of low thermal

expansion material of this type happened to be in 1897 by Guillaume and it

was the famous industrial alloy InVar (Fe.64Ni.36) [41]. Since then there are

many known magnetic materials which exhibit NTE include alloys (GdAgMg

[6] ), iron based alloys ( Nd2Fe17Nx[42], Gd2Fe17[43]), oxides ( (La0.8Ba0.2)MnO3

[44]), sulphides(CdCr2S4 [45]), fluorides (perovskite MnF3 [5] ) and nitrides

(antiperovskite manganese alloy based nitrides [46]). These materials display

a variety of unusual mechanical properties such as large, tunable CTE over

a considerable temperature span. An excellent review of NTE in functional

materials can be found in literature [47]

1.3.2 Negative thermal expansion from framework dynamics

Besides NTE from phase competition, there also exists a growing class of mate-

rials with strong, isotropic, robust and thermally persistent NTE that originates

from vibrational mechanism, or in other words intrinsic structural degrees of

freedom. NTE of this type has recently been described as structural negative

thermal expansion (SNTE) [48].

SNTE is a fascinating and growing field of condensed matter physics due

to the rarity of the phenomenon, stunning display of unconventional lattice

13

Figure 1.3.3: NTE in magnetic materials. (a) Temperature dependence of the unit-cell volume of MnF3 . The Neel temperature, TN is shown. From [5]. (b) Relative length changes L/L0 of ferromagnet GdAgMg for various magnetic fields. From [6]

dynamics, and strong potential for structural applications where dimensional

stability is required. This type of NTE phenomenon refers to the unusual

tendency for materials to shrink when heated as a property of bond network

topology and the associated fluctuations [49, 50, 51] which is distinct from NTE

arising from electronic or magnetic degrees of freedom described in section

1.3.1.

SNTE is most often discussed in connection with transverse fluctuations of

a linkage between volume defining vertices, which may accompany the libra-

tional (rocking) vibrations in rigid bonds or hindered rotational motion of rigid

polyhedral subunits. The most studied example that shows this type of be-

havior is ZrW2O8 (ZWO) [7, 52, 53, 54, 55, 56]. This cubic material has a large

unit cell, containing 44 atoms in the form of corner linked ZrO6 octahedra and

14

Figure 1.3.4: Negative thermal expansion in ZWO. Filled circles represent neutron diffraction data while open circle represent dilatometry data. Taken from [7].

WO4 tetrahedra. The NTE behavior is strong (Figure 2.3.9) in ZWO ( αV = -27.3

x 10−6/K up to 400K) compared to most of NTE materials of this class and re-

ported over wide range of temperature range (0.3-1050 K). The ZrO6 octahedra

and WO4 tetrahedra connect via the corner O atom, but one of the O in WO4 is

not connected to another unit and the origin of the NTE comes from transverse

vibration of Zr - O - W bond [57]. At the same time, the NTE in ZWO survives

even after a phase transition occurs at 430 K, but the volumetric thermal expan-

sion coefficient decreases to -18 x 10−6/K. Well-known categories of materials in

which the NTE behavior has been attributed to vibrational mechanisms include

metal cyanides [58], various zeolite frameworks [59], A2M3O12 series [60, 61],

ZWO family[7, 62], ZrV2O7 family[63, 64], Prussian blue analogues[65], MOF-5

materials [66, 67] and metal fluorides [68].

15

1.4.1 Grneisen theory and thermal expansion

As introduced by Germen Physicist Eduard Grneisen [69, 70], Grneisen theory

assumes that the phonon frequencies of a crystal are modified as the volume

changes. The changing frequencies would allow calculating thermodynamic

functions with in harmonic approximation. This approach is known as quasi-

harmonic approximation. See reference [71] for more details.

Within Grneisen theory, for a crystal with many normal modes, the mode

Grneisen parameter is defined, which explains the effect that changing the vol-

ume of a crystal lattice has on its vibrational properties, and as a consequence,

the effect that changing temperature has on the size or dynamics of the lattice.

Since thermal expansion is a result of the anharmonic nature of bonds, quan-

tification of the anharmonicity in a solid can be achieved with mode Grneisen

parameter, γ(q)i. The mode-dependent Grneisen parameter for a phonon mode

i at a reciprocal lattice point q can be defined as

γ(q)i = − ∂ logω(q)i

∂ log V (1.4.1)

where V is the unit cell volume, and ω(q)i is the frequency of the ith mode of

vibration, which itself is a function of a wave vector q in the BZ.

Equation 1.4.1 implies that for a NTE material, γ(q)i is negative, for modes

16

soften with increasing temperature and positive, for modes stiffen with in-

creasing temperature. The overall expansion behavior of a material depends

on the combined contributions from all modes, therefore materials with neg-

ative mode Grneisen parameters are not necessarily NTE materials. Often

thermal expansion is quantified by mean Grneisen parameter, obtained by

integrating Equation 1.4.1 over all modes:

γ = − αVBV

CV (1.4.2)

where B is bulk modulus and CV is constant volume heat capacity. As B,CV,

and V are positive for materials in thermodynamic equilibrium, NTE materials

necessarily possess a negative mean Grneisen parameter.

1.4.2 Rigid unit mode picture

Studies have shown that the lattice vibrations responsible for NTE in ZWO

are in the energy scale of around 2 meV [55, 50, 72, 73]. The bond stretching

and bond bending modes are mostly frozen at this energy scale and vibrations

which respect and maintain internal polyhedral distances and bond angles

have special significance. The WO4 tetrahedral stretching and bending modes

are not thermally excited at the low temperatures where NTE begins, [56]

suggesting a hierarchy of energy scales: stiff bond stretching, intermediate

bond bending, and a set of low- energy external modes of rigid polyhedra

17

units called rigid unit modes (RUMs). The latter set may be supported at low-

energy only in certain regions of reciprocal space which are particular to the

system under consideration.

The RUM model was first used to explain the displacive phase transitions in

silicates [74, 75]. It was developed to describe the behavior of materials with

crystal structures that can be described as frameworks of linked polyhedra

(examples are ScF6 octahedra in ScF3 and WO4 tetrahedra in ZWO). Vallade

and coworkers [76] have shown that the softening of an optical mode nearby

an acoustic phonon causes the phase transition of the material quartz and the

whole phonon branch has a low frequency at each k values, hence must be

associated with RUMs not only at one k value, but along the whole branch.

The idea of RUMs acting as soft modes for displacive phase transition was

later developed for silicates using a split atom method.

The RUM model has given a number of other new insights and most impor-

tantly it has also been used to explain the origin of negative thermal expansion

in framework structures. Phonons described by RUM model are associated

with collective motion of polyhedra and those collective motions cause atomic

displacement without distorting the polyhedra. Therefore these modes are

often identified as NTE modes in SNTE materials. Usually the polyhedra vi-

brational energies are very high when they are distorted compared with the

energy when they are not distorted. As a result, we generally expect RUM

modes to have low energies. For ZWO the manifold of momenta supporting

18

RUMs is very complex, as identified through classical calculations [54] using

split atom approach. Simplest case of RUMs associated NTE is described in

cubic lattice systems ScF3 and ReO3 and more importantly their RUMs corre-

spond to simple momentum space manifolds. ScF3 has only four atoms per

unit cell and forms with corner linked octrahedra of ScF6. High symmetry

points of Brillouin zone (BZ), corresponds to in phase rotation of each stack of

octrahedra (M point) and out of phase rotation of each stack of octrahedra (R

point) defines the boundaries of RUM in ScF3 material. Please see Figure 5.1.1

for a better view on this.

Welches and coworkers have developed a simple qualitative picture explaining

NTE [77] in ReO3 like structures. It is related with geometrical frame work and

is associated with the rotation of stiff structural units or bond bending of the

shared corner atom of the polyhedra units by preserving the rigid unit structure

(RUM). For simplicity the rotation of a 2D perovskite (2D frame work of linked

squares) is considered and the important point is that the area or lattice constant

is reduced by the rotation as a straightforward geometrical effect(Figure 1.4.1).

Considering the potential energy of rotation due to thermal fluctuations, 1 2

Iω2 θ2 T =

1 2

kBT2 where I is the moment of inertia of the units, ω2 is average or Einstein

frequency for the rotations, θ2 T is the equilibrium fluctuating value of θ2 at

temperature T, kB is Boltzmanns constant. Considering the lattice area reduc-

tion, from A0 to A0 cos2 θ the lattice constant obeys the relation a = a0(1 − ηaθ2)

and the expression a a

= − ηakBT Iω2 is obtained, which then reduces to CTE

19

Figure 1.4.1: Rotation of 2D perovskite leads to an area reduction.

αL = − ηakB

Iω2 . Here ηa is identified as geometrical constant which is equal to

unity in this case. Chapter 5 discusses a model that we developed to approx-

imate the staggered rotation in 2D square lattice and proves that the above

constant equals to 1/2 in a 2D lattice with few squares, where harmonic wave

limit is applied and 2/3 in a lattice with large number of square units, where

circle wave limit is applied.

As shown the geometrical effect on the CTE leads to a negative CTE. At the

same time since the frequency of modes appears at the bottom of the CTE it

resembles that the softer modes contribute more to the CTE. A particularly

soft dynamic distortion of this structure preserves bond lengths and internal

polyhedral bond angles while decreasing the volume of the time-averaged

structure as the vibrational amplitude is increased through thermal activation.

This classical picture has been widely discussed in general reviews of the NTE

20

phenomenon[78, 79, 80, 81].

1.4.3 Tension effect and NTE

SNTE is commonly described using a mechanism called tension effect which is

thoroughly discussed in the review [8]. The simplest form of the tension effect

considers a linear molecule which consists of three atoms. As the center atom

of the linkage move transversely, the corner atoms move towards each other,

assuming the bonds are rigid. Applying this into three dimensional (3D) struc-

ture immediately implies that the structure decreases it’s dimensions, hence

NTE. As the corner atoms of the linkage move further away from each other

the amplitude of the transverse fluctuation of the center atom decreases and

results in increasing volume. This results in increasing stretch or the tensions

of the bonds, suggesting negative Grneisen parameter. Thermal ellipsoids dis-

played by 3D systems such as ScF3 and ReO3 are consistent with the tension

effect and the mechanism is most useful in interpreting the NTE of CN− frame-

work structures such as AgCN, AuCN, CuCN and Ni(CN)2. RUM model is a

special case discussed under tension effect.

1.4.4 Thermodynamics of NTE materials

A study [82] has shown that for materials with positive compressibility and

NTE, the first law of thermodynamics reads as dQ = dU−PdV. The author has

mathematically proved, that the first law of thermodynamics (dQ = dU + PdV)

holds true only if either both the compressibility and thermal expansion are

21

Figure 1.4.2: Representation of the tension effect. A linear linkage of three atoms is shown in left. This can distort such a way that the central atom displaces transverse direction or the two end atoms displace in opposite ways. In both cases the bonds stay in rigid and the two end atoms move inwards in the vertical direction. Taken from [8]

negative or both of them are positive. A different [83] study has proposed

the isentropic (constant entropy) volume expansivity, αV = (1/V)(∂V/(∂T)S

for materials with NTE instead of standard definition of isobaric (constant

pressure) CTE, αV = (1/V)(∂V/(∂T)P.

There are plenty of materials found to be possessing NTE property and thou-

sands of literature have been published directly or indirectly related with NTE

phenomenon, but only a handful numbers of thermodynamic analysis on NTE

materials are found in literature. So readers who are interested would find it

is worth working in this field.

1.5 Perovskites

22

Perovskite oxides, a class of solid materials with chemical formula ABO3, con-

tains examples of perhaps every possible type of material behavior. Underpin-

ning the competing interactions behind this diversity are fascinating cascades

of structural transitions associated with tilts of the BO6 octahedra, which are

strongly influenced by the A-site ions through geometric tolerances[84, 85].

A-site-free perovskites based on oxygen are rare, as the B ion must take on the

extremal +6 valence state, and the only known instance is ReO3. A moderately-

sized NTE effect occurs at low temperature in this material[86] and can be

understood in terms of a model of rigid unit modes (RUMs) described in sec-

tion 1.4.2. Though that is the case with oxides, A site free perovskite fluorides

or in other words MF3-type structures are not rare because of the common

trivalent(+3) state found in most of the metals in the periodic table, especially

among transition metals and lanthenides.

1.6 Trifluorides and their structures

Figure 1.6.1 shows a global structural phase diagram of MF3 perovskites, where

M is a +3 metal ion. For large (rS > 0.85A) ionic radius rS (Shannon), fluorine

ions can pack around the M ion with high F coordination up to n=8 or 9 in com-

mon large-gap optical materials of orthorhombic and tysonite type structures

which are commonly formed with rare earth metal ions.

Order-disorder type second order phase transitions has been reported for LaF3

- NdF3[87] (refer Figure 1.6.1), from low temperature trigonal(P3c1) to high

23

Figure 1.6.1: Global structural phase diagram of MF3 type perovskites.

temperature hexagonal (P63/mmc) phases which both are two modifications

of tysonite type structure[88]. SmF3 - GdF3 crystallize from melt to tysonite

type structure and upon cooling they transform into orthorhombic(Pnma) β-

YF3 [89] type structure. Structural phase transitions occurred in TbF3, DyF3

and HoF3 are accounted for some sort of impurity[90, 91, 92] in the system and

no transition has been reported for pure systems. ErF3 - YbF3, LuF3 and YF3

yield a new high temperature form of α-YF3 type[92].

Below rS < 0.8A, perovskites form with simple-cubic symmetry(Pm3m) at high

temperatures. At low rS, and among the 3d metal trifluorides, a structural

cubic-to-rhombohedral(R3c) phase boundary is apparent, with the exception

24

of MnF3. ScF3 is the only trifluoride with cubic symmetry at room temperature

and can be considered to be the standout among all and will be discussed

thoroughly through out the thesis.

1.7 Scandium trifluoride(ScF3)

Recently, nonmagnetic ionic insulator ScF3 has drawn particularly intense at-

tention in the chemistry community[9] as the first instance of a perovskite-

structured material with strong, isotropic, and thermally persistent NTE, a

distinction which no longer appears to be an isolated case[93]. ScF3 displays

strong NTE (-42 ppm/K < αV < 0) over a temperature window of 1000 K, but is

also unusual in its lack of any type of phase transition whatsoever within the

solid state.

Cubic ScF3 has 4 atoms per unit cell and consists of corner-inked octahedra

which fill space in three dimensions with unit cells a = b = c. The high

symmetry points in the first Brillouin zone (BZ) in reciprocal space are labeled

zone center Γ(0, 0, 0), zone face center X (2π/a(1/2, 0, 0)), zone edge center

M(2π/a(1/2, 1/2, 0)), and zone corner R(2π/a(1/2, 1/2, 1/2)). Sc has the longest

Shannon effective ionic radius of all 3d transition metal trifluorides, and the

lattice dimension parameter a = 4.02 Å at room temperature is very close to

twice the sum of these radii for Sc (0.745 ) and F (1.19 Å), suggesting chemical

25

1.7.2 Pressure induced phase transition in ScF3

Cubic ScF3 further stands out among substances in that it has the most stable

structural phase of any known solid trifluoride, retaining cubic symmetry from

its high melting point >1800 K to <0.5 K[9, 94]. A finite-temperature cubic to

rhombohedral (c-r) transition can be induced however through application of

slight pressure [95, 96] (<0.2 GPa ∼ 2000 atm), chemical substitution of Ti[20],

Al[19], or Y[97] for Sc, and even by the weak stresses induced by polymeric

impregnation of powder samples[21], suggesting that the quantum nature of

the cubic phase at low temperature is delicate and susceptible to even mild

perturbations.

X-ray diffraction [95, 9] and Raman spectroscopy[95] results have revealed

that at room temperature ScF3 undergoes a pressure induced phase transition

from c-r between 0.5 and 0.8 GPa and rhombohedral to orthorhombic structure

above 3.0 GPa. As suggested by the authors[95] the first transition point which

is quite low as hydrostatic pressure is the result of disturbance of the balance

between short-range dipoledipole(of fluorine ions) and long-range Coulomb

interactions which is related to rotation of the ScF6 octahedra around a threefold

axis. The rotation of octahedra corresponds to R = π/a(1, 1, 1) point in cubic

phase BZ and the c-r phase transition occurs due to condensation of this mode

(Figure 1.7.1).

Observed pressure dependence of the transition temperature is dTc/dp ∼ 525

K/GPa [9, 95, 96]. The c-r phase transition in ScF3 is never realized down to 0.4

K [94] in atmospheric pressure and using inelastic x-ray scattering (Chapter:2)

results, we estimate that pressures as small as 740 bar = 0.074 GPa would be

sufficient to drive the transition upward to 0 K. The sensitivity of the phase

boundary suggests that the nature of the cubic phase is delicate at low temper-

ature and susceptible to even mild perturbations [21, 20, 20, 19]. Section 2.3.10

further discusses this.

If suitable substrates of ScF3 are developed, new functionalities may be reached

in film synthesis, as cooling from the growth temperature would effectively

stretch epitaxial films. Significant efforts in the physics groups of Profs. Barrett

Wells in Physics Department have already produced thin films of NTE ScF3

[98]. Thin films of ScF3 are grown using pulsed laser deposition, and while

large fraction of a film is having very good epitaxy and small mosaic, remaining

regions are polycrystalline. Unique features of this material such as large band

gap, non-oxide nature, poor adhesion under pressure and high saturated vapor

pressure remain as significant challenges to overcome.

1.7.3 Electronic structure of ScF3

In formation of ScF3, from a scandium atom and a fluorine atom, the scandium

atom loses its three valence electrons (and turn to Sc+3 ) to three fluorine atoms

(and form F−), which each of the fluorine has just enough space to accept it. We

27

Figure 1.7.1: Pressure-temperature phase diagram for ScF3. The dashed line is a guide to the eye. Two layers of octahedra in both the cubic and the rhombo- hedral ReO3 structures (viewed along [111]) are shown. Upon pressurization, octahedral tilts fold the structure so that it is more compact and reduce the symmetry from cubic to rhombohedral. Taken form [9]

must realize that unlike other 3d type transition metal trifluorides Sc+3 in ScF3

has 1s2 2s2 2p6 3s2 3p6 4s2 3d0 configuration and hence no free d electrons. One

consequence is that ScF3 has no local moment magnetism and no free electrons,

implying that the available degree of freedom are purely lattice origin.

The band structure of ScF3 clearly shows a band gap of at least 8 eV which

is an indication of strongly bound valence electrons and empty conduction

band, pernitting classification as an ionic insulator. It should be noted that

ReO3 (introduced in 1.5), a material isostructural to ScF3, happens to be a good

28

metal. The vastly different electronic structures of otherwise similar materials

might be interesting to further investigate.

Since both materials are SNTE materials, it is meaningful to compare the elec-

tronic structures of each with its own distorted structure. Using first principle

calculations, a comparative study [99] has been carried out and the electronic

band structure of distorted ReO3 (O atoms are displaced perpendicular to Re-

O-Re bond) has shown a small destabilization of the flat conduction band

compared with conduction band of non-distorted structure. The atomic dis-

placement was attributed to formation of antibonding orbitals and the authors

conclude that this results in destabilizing the distortion of ReO3 structure. On

the other hand the electronic band structure of distorted ScF3 structure hardly

changes from its non distorted counterpart. Therefore it is concluded that the

ScF3 favors the distortion more than that of ReO3 and as a result the CTE of

ScF3 (αV = -42x10−6/K in 60 K to 110 K temperature window and ∼ -25x10−6/K

at 300 K) is larger than ReO3 (αV = -7.68x10−6/K in 5 K to 300 K temperature

range).

1.8 Motivation

A central question in the study of SNTE is whether basic structural mechanics

principles and intuition can be applied to guide discovery of new materials

that display this anomalous effect. For example, metallic ReO3 and insulating

ScF3 with open perovskite structure display SNTE over a wide range of tem-

29

peratures, but why do other open perovskites most commonly exhibit positive

thermal expansion (PTE)? or can composite materials be formed with thermal

expansion over a wide temperature window, or do stresses inevitably shift the

structural phase to one with PTE? Why is SNTE so rare, inevitably yielding to

PTE in response to disorder and application of pressure?

In pursuit of conceptual control of the phenomenon, innovative approaches

have been offered which link thermally activated transverse vibration of struc-

tural units to a tendency to draw in lattice dimensions. Rigid unit approaches

view polyhedral molecular units (i.e., metal-anion tetrahedra and octahedra)

rather than ions as the fundamental building blocks of a material and attempt

to link the states built from rotational zero modes of the free molecules to the

low-energy modes of the crystal. In this view, intramolecular degrees of free-

dom are effectively integrated out, and the nature of their coordinated motion

as a function of lattice topology and connectivity is the central feature of SNTE.

New discoveries of robust SNTE have reinvigorated the field and raised the

question of whether strict molecular rigidity is an appropriate starting point

or if, instead, it is more appropriate to consider only the rigidity of the stiffest

bonds in a view of the materials as a framework of struts.

30

2.1 Introduction to Inelastic X-ray Scattering

Inelastic x-ray scattering (IXS) is an experimental technique which is used to

investigate distinct forms of material dynamics. In simple words, a collection of

a photon is sent in and the energy and the momentum of the scattered photons

are analyzed which carry information of disparate excitations of the material.

These excitations basically are differentiated by their energies and a schematic

is provided in Figure 2.1.1.

Figure 2.1.1: Excitations that may probe using IXS, From [10]

31

We can identify several distinct methods used in order to probe those excitations

and since there are no sharp boundaries among excitations energies, some of

them may be probed using more than one technique. Table 2.1.1 lists some of

the techniques that fall under the broad interpretation of the IXS.

Technique Incident photon energy

tum density Magnetic Compton 100 keV eV Density of un-

paired spin RIXS(Rasonance) 4-20 keV 0.1 - 50 eV Electron structure

and excitations SIXS(Soft x-ray) 0.1-2 keV 0.01 - 5 eV Electronic and

magnetic struc- ture and excia- tions

NIS(Nuclear IXS) 10-30 keV 1 - 100 meV Element specific phonon and Density of state (DOS)

X-ray Ramam 10 keV 50 - 1000 meV Edge structure, Bonding, Valence

NRIXS 10 keV 0.01 - 10 eV Electronic struc- ture and excita- tion

IXS 10-25 keV 1 - 100 meV Atomic dynamics and phonon dis- persion

Table 2.1.1: List of techniques broadly grouped under the heading of Inelastic X-Ray Scattering.From[10]

2.1.1 IXS advantages over other spectroscopic techniques

One of the significant advantages of IXS is the access to small samples. The

32

synchrotron radiation of high flux and brilliance is capable of focusing the

beam to ∼ 100 microns diameter easily. Even ∼ 10 microns in diameter can

be achieved with some losses. The facts that incoming x-ray photon energy

of ∼ 20 keV is significantly higher than the measured energy transfer of ∼

1-200 meV and the energy and momentum of photon is directly proportional

to each other lead to other compelling advantageous of using IXS such as

decoupling of the energy and momentum transfer, achieving high momentum

resolution and independence of energy resolution from energy transfer. The

Thompson cross section for x-rays is smaller than the absorption scattering

cross section at least by one order of magnitude. This could prevent multiple

scattering from the sample and incoherent scattering at higher energies by only

penetrating into the top 0.01 or 0.1 mm of the sample. Therefore most materials

have very short attenuation length for x-rays which eventually results in lower

background signal as well. But in case of neutron, the scattering cross section

dominates hence multiple scattering can be a problem. On the other hand

higher absorption cross section in x-rays could easily leads to radiation damage

of the material. Nevertheless, it is worthwhile to mention that neutron holds

the edge when higher energy resolution is needed but some of the samples can’t

be measured using neutron scattering or diffraction experiments as they highly

absorb neutrons. Some of the common examples are Cadmium, Samarium and

Europium.

Next section in current chapter is dedicated to elaborate general scattering

33

theory using both classical and quantum mechanical perspectives. It will be

followed by a discussion on probing phonons from a theoretical point of view.

In last section, I will discuss the IXS experimentation to investigate the lattice

dynamics, especially, phonons in crystalline material ScF3.

2.2 Scattering theory

Consider scattering of an x-ray beam from two atoms in an arbitrary lattice

planes of a sample which are separated by distance r. Unlike in x-ray diffraction

the lattice planes can be nonparallel. Lets assume the incoming x-ray wave

vectors are parallel and are denoted by −→ ki . The scattered wave vectors(parallel)

are −→ k f . See Figure 2.2.1 for clear view.

Figure 2.2.1: X-ray scattering from an arbitrary atoms

In order to determine whether the interference is constructive or destructive,

we need to figure out the phase difference between two waves. phase difference

can be obtained by considering the path length difference and can be written

34

as

and using vectors we may write

−→ ki . −→r = |

l1 = λ

Therefore the path length difference can be written as

l = λ

and the phase difference is given by

l 2π λ

−→ Q =

−→ k f − −→ ki (2.2.10)

The scattering wave vector, −→ Q and the spatial arrangement of the atoms in the

sample are key factors when determining the signal at the detector. The spatial

positioning of atom is important since it determines the tendency of sample to

scatter the incoming wave. We can introduce the density of scattering atoms

in the sample to be ρ(−→r ) and assume the scattering density depends on the

36

spatial arrangement of atoms.

Figure 2.2.2: Radiation from source (S) to detector (D) via the sample

Using plane wave approximation and incorporating all above variables, an

expression for the amplitude of the signal at the detector(scattering wave aml-

pitude), fD from a wave emitted by point at tip of the −→r can be written as,

fD ∝ ρ(−→r )ei( −→ ki− −→ k f ).−→r (2.2.11)

fD ∝ ρ(−→r )e−i −→ Q.−→r (2.2.12)

This is specifically derived for one particular point in the sample. Therefore to

calculate the total amplitude at detector we need to integrate over the sample

volume.

37

fD ∝

where V is the total volume of the sample.

Fourier transformation of scattering density leads to the expression

ρ( −→ Q) =

−→ Q.−→r d−→r (2.2.14)

which is similar to the amplitude of the signal at the detector.

To describe the scattering density within one unit cell let us assume the atoms

in the unit cell don’t interact with each other and have their own local scattering

density ρ j( −→ r′ ) where

−→ r′ = −→r − −→r j (2.2.15)

Figure 2.2.3: Reflection geometry where the blue solid circle represents the jth

atom where −→r j and −→r initiate at the unit cell origin

38

ρ j( −→r − −→r j ) (2.2.16)

Now rewriting the total scattering, plugging ρ j( −→ r′ ) and multiplying by 1 =

ei −→ Q.−→r j e−i

−→ Q.−→r j

−→ Q. −→ r′d −→ r′ (2.2.17)

Here the integral term is known as atomic form factor f j( −→ Q) which is a property

of atoms themselves and the summation term ∑

j ei −→ Q.−→r j depends on where the

atoms are located in the lattice. Finally the intensity of scattered beam is given

by

In previous section I have formulated a mathematical expression described

scattering from arbitrary atoms instantaneously at a given time. But we can ex-

tend our analysis further to consider scattering from sample atoms at different

39

times. This of course, results in a phase shift in the scattering wave.

Redefining the scattering density in momentum space and introducing phase

shift e−iωt,

ρ( −→ Q, t) =

Averaging all time to get the total scattering

ρ( −→ Q, ω) =

Writing the intensity of the scattering

S( −→ Q, ω) =

∫ ρ(− −→ Q, t)e−iωtdt (2.2.21)

Shifting t by t + t′

S( −→ Q, ω) =

Performing an average over all time origins

S( −→ Q, ω) =

∫ ρ( −→ Q, 0)ρ(−

40

S( −→ Q, ω) =

−→ Q.−→r k(t)

e−iωtdt (2.2.24)

This is a critical equation in IXS which carries both spatial and time evolution

information about excitations of the system and known as dynamical structure

factor. More importantly for us the signal or the spectra collected in IXS

experiment is directly proportional to dynamic structure factor(S( −→ Q, ω)) of the

material.

Let me start by considering the electron-photon interaction Hamiltonian. Con-

ventionally it can be separated into two terms H0 and Hi, where non interacting

term reads

and electron - photon interaction term is given by

Hi = ∑

j

e2

2mc2

−→p j (2.2.26)

While −→ A and V denotes the electromagnetic field vector and scalar potentials,

41

the electron momentum and position are denoted by−→p and−→r . In Hamiltonian,

Hi the first terms with A2 term dominates in nonresonant scattering processes

while the second term leads in resonant scattering (case where the incoming

energy is tuned into absorption edge of the atom). The nonresonant scattering

cross section depends on dynamic structure factor and has the form of Equation

2.24. Since we only deal with nonresoannt scattering, from here onwards I

would only take H(1) i =

∑ j

e2

2mc2

−→ A2(−→r j ) term into consideration.

Introducing the photon creation (a†kα) and annihilation (akα) operators the vector

potential can be written as

−→ A(−→r ) = L−3/2

−→ k −→r ) (2.2.27)

where ωk, α and k denote the angular frequency, polarization and wave vector

of photon respectively. L3 is normalization box volume.

Let us now consider photon in three dimensional box of side L. The photon

states are quantized and only allowed k values given by 2π/L(nx,ny,nz) where

nx, ny and nz are integers.

Any possible final-state wave-vector k corresponds to a point in wave vector

space with coordinates (kx, ky, kz). Then we can define the density of k states

(number of k points per unit volume) to be L3/(2π)3. In three dimensional

system the k space volume between k′ and k′ + dk′ is 4π2k′2dk′. Therefore the

number of k states in the r

Follow this and additional works at: https://opencommons.uconn.edu/dissertations

Recommended Citation HANDUNKANDA, SAHAN UDDIKA, "Lattice Dynamics Studies of Negative Thermal Expansion Due to Two Low-temperature Lattice Instabilities." (2018). Doctoral Dissertations. 2021. https://opencommons.uconn.edu/dissertations/2021

Low-temperature Lattice Instabilities

ABSTRACT

Here I present a complete study of lattice dynamics of negative thermal ex-

pansion (NTE) material Scandium trifluoride (ScF3) and discovery of NTE in

mercurous iodide (Hg2I2). An inelastic x-ray scattering (IXS) study of ScF3

reveals copious evidence of an incipient soft-mode instability indicating that

the T=0 state of ScF3 is very close to a structural quantum phase transition

(SQPT). Is the anomalously strong and thermally persistent NTE behavior of

ScF3 a consequence of the SQPT? In order to address that, we have explored

the coefficient of thermal expansion (CTE) and soft mode behavior of a sec-

ond stoichiometric compound, situated near a SQPT. A detailed side-by-side

comparison of the metal trifluorides and mercurous halides suggest strong

similarities and a generic connection between the fluctuating ground state

of incipient ferroelastic materials and SNTE. We find experimental evidences

Sahan Handunkanda - University of Connecticut - 2018

for two- dimensional nanoscale correlations exist at momentum-space regions

associated with possibly rigid rotations of the perovskite octahedra of ScF3.

The discussion is extended by addressing the extent to which rigid octahedral

motion describes the dynamical fluctuations behind NTE by generalizing a

simple model supporting a single floppy mode that is often used to heuris-

tically describe instances of NTE. Temperature-dependent infrared reflection

measurement on single crystal ScF3 is performed to understand the zone cen-

ter lattice dynamics of ScF3. In addition, I also carried out an instrumentation

development project in the laboratory at the Department of Physics which will

be briefly discussed in the last chapter.

Lattice Dynamics Studies of Negative Thermal Expansion Due to Two

Low-temperature Lattice Instabilities

M.S. Physics, University of Connecticut, Storrs, CT, 2014 B.S. Physics, University of Colombo, Sri Lanka, 2009

A Dissertation Submitted in Partial Fulfillment of the

Requirements for the Degree of Doctor of Philosophy

at the University of Connecticut

2018

Lattice Dynamics Studies of Negative Thermal Expansion Due to Two

Low-temperature Lattice Instabilities

Major Advisor Jason Hancock

Associate Advisor Barrett Wells

Associate Advisor Douglas Hamilton

University of Connecticut 2018

iii

ACKNOWLEDGEMENTS

This thesis would not have been possible without collective effort and co- operation of many people. First of all, I would like to express my deepest appreciation to my PhD advisor Dr. Jason Hancock. I am greatly thankful for the faith that my advisor had on me from the day we first met, especially by welcoming me as his first graduate student. Throughout my PhD, I enjoyed and learnt from his knowledge and expertise in condensed matter research. He has given enormous encouragement and assistance while being patience with me over the past six and half years, something I truly appreciate. His characteristic traits eventually helped me to develop as a skilled physicist.

I also offer my sincere gratitude to Dr. Barrett Wells and Dr. Douglas Hamilton who served me as associate advisors. Apart from Dr. Wells’s proficiency and valuable discussion on my research I am also thankful to Dr. Wells for recom- mending me to talk with at the time new faculty member, Dr. Hancock about prospective research opportunities. I would like to thank Dr. Hamilton for his advise and encouraging words on writing which is the key to a successful scientific career.

I would like to express my gratitude to the beamline scientist Dr. Ayman Said at sector 30, Advanced Photon Source, Argonne National Laboratory for supporting us while we were taking our data on Scandium trifluoride samples. He provided a great amount of technical support during multiple beamtimes, which I never forget and greatly appreciate.

Successful experimentation is never possible without having quality samples. My special thanks goes to Dr. Vladimir Voronov in Kirensky Institute of Physics in Russia for proving us isotopically pure, single-crystalline Scandium triflu- oride samples and Dr. Sudhir Trivedi in Brimrose Technology Corporation, Sparks, Maryland for proving us single crystalline Mercurous Halide samples.

Theoretical collaborates are a vital part of a research study. The discussion we had and their insight on interpreting the experimentation results helped us to communicate and efficiently present the research findings and I would take this opportunity to thank the team led by Dr. Peter Littlewood then director of Argonne National Laboratory, Dr. Gian Guzman-Verri, and Dr.Richard Brier- ley in Yale University.

My sincere thanks goes to Dr. Joseph Budnick, Dr. William Hines, Dr. Boris

iv

Sinkovic, Dr. Gerald Dunne and Dr. Gayanath Fernando for the valuable con- versations that we had on our experimentation results. I appreciate Dr. Ilya Sochnikov and Dr. Diego Valente for accepting the invitation to take a part in my dissertation committee on such short notice. I would also like to thank to Dr. Dave Perry, someone who is always willing to help, especially when I need to figure out mechanical part necessary for my research work. Special thanks goes to Alan Chasse, the machine shop engineer for making all the necessary mechanical parts used in instrumentation development. I would also like to thank the former office staff Dawn, Kim and Babara as well as the current office staff in Physics, Micki, Anna, Caroline and Alessandra for their support in administrative works.

I would like to thank all my group members Erin Curry, Donal Sheets and Connor Occhialini whom I had a great time working with and had a lot of fun during my PhD in and out of the laboratory. The support and encouragement provided by Sri Lankan community at UConn, my batch mates Niraj, Zhiwei, Udaya, Susini, Katya and Dale at the difficult time during my stay at Storrs are hugely appreciated.

Last but not least I thank my dear parents, sister and my beloved wife Awanthi for their endless support and love provided me during the past few years.

v

TABLE OF CONTENTS

Ch. 1 : Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 1.1. Thermal expansion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 1.2. Lattice Dynamics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2 1.3. Negative thermal expansion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9 1.3.1. Negative thermal expansion from phase competition . . . . . . . . . . . . . 10 1.3.2. Negative thermal expansion from framework dynamics . . . . . . . . . . 13 1.4. Theoretical consideration of negative thermal expansion . . . . . . . . . . . 16 1.4.1. Grneisen theory and thermal expansion . . . . . . . . . . . . . . . . . . . . . . . . . 16 1.4.2. Rigid unit mode picture . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 17 1.4.3. Tension effect and NTE . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 21 1.4.4. Thermodynamics of NTE materials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 21 1.5. Perovskites . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 22 1.6. Trifluorides and their structures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 23 1.7. Scandium trifluoride(ScF3) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 25 1.7.1. Negative thermal expansion in ScF3 . . . . . . . . . . . . . . . . . . . . . . . . . . . . 25 1.7.2. Pressure induced phase transition in ScF3 . . . . . . . . . . . . . . . . . . . . . . . 26 1.7.3. Electronic structure of ScF3 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 27 1.8. Motivation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 29

Ch. 2 : Lattice dynamics study of ScF3 using inelastic x-ray scattering . . . 31 2.1. Introduction to Inelastic X-ray Scattering . . . . . . . . . . . . . . . . . . . . . . . . . . 31 2.1.1. IXS advantages over other spectroscopic techniques . . . . . . . . . . . . . . 32 2.2. Scattering theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 34 2.2.1. Dynamic structure factor (S(

−→ Q, ω)) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 39

2.2.2. Quantum mechanical perspective . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 41 2.2.3. Scattering cross section . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 48 2.2.4. IXS for phonons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 49 2.2.5. Scattering from phonons in theoretical perspective . . . . . . . . . . . . . . 51 2.3. Inelastic X-ray Scattering on ScF3 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 55 2.3.1. The Experiment . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 56 2.3.2. Single crystal ScF3 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 56 2.3.3. Lattice parameter measurement . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 61 2.3.4. Phonon dispersion relation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 62 2.3.5. M-R branch and NTE . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 63 2.3.6. M-R branch and phase transition . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 64 2.3.7. Central peak of ScF3 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 67 2.3.8. What causes central peak? . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 68 2.3.9. Central peak of ScF3 and mode softening . . . . . . . . . . . . . . . . . . . . . . . . 72

vi

2.3.10. Quantum phase transition in ScF3 and phase transitions in other transition metal trifluorides . . . . . . . . . . . . . . . . . . . . . . . . . . . . 76

2.3.11. ScF3 systems and disorder . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 78 2.3.12. Transverse motion of F atoms . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 81 2.3.13. Elastic parameters of ScF3 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 82 2.3.14. Modeling IXS data using Damped Harmonic Oscillator(DHO) . . . . 86

Ch. 3 : Comparative study of two incipient ferroelastics, ScF3 and Hg2I2 92 3.1. Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 92 3.2. Low-T structure and scattering evidence for the IFE behavior of

Hg2I2 and ScF3 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 94 3.3. Discussion and SNTE material design principles . . . . . . . . . . . . . . . . . . . 98

Ch. 4 : Thermal Diffuse Scattering on ScF3 . . . . . . . . . . . . . . . . . . . . . . . . . . . 106 4.1. Introduction to diffuse scattering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 106 4.2. Diffuse Scattering study of single-crystalline compound ScF3 . . . . . . . 107 4.2.1. Experiment . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 107 4.2.2. Negative thermal expansion of ScF3 and diffuce scattering . . . . . . . 108 4.2.3. Results and discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 110

Ch. 5 : Two dimensional constrained lattice model to study ScF3 lattice . 114 5.1. Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 114 5.2. Two-dimensional constrained lattice model . . . . . . . . . . . . . . . . . . . . . . . 115 5.3. Application of model to experimental results . . . . . . . . . . . . . . . . . . . . . . 121

Ch. 6 : Infrared study of ScF3 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 125 6.1. Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 125 6.2. Measurements . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 126 6.3. Lorentzian model fitting . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 127 6.4. Factorized model fitting . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 128 6.5. Zone center modes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 132 6.6. Infrared measurement results . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 134 6.6.1. Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 137

Ch. 7 : Resonant Ultrasound Spectroscopy . . . . . . . . . . . . . . . . . . . . . . . . . . . . 147 7.1. Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 147 7.2. Elastic properties and constitute equations . . . . . . . . . . . . . . . . . . . . . . . . 148 7.2.1. Symmetries in cubic systems and other important properties . . . . . . 151 7.3. Resonant ultrasound spectroscopy fundamentals . . . . . . . . . . . . . . . . . . 154 7.4. ScF3 sample and RUS setup used . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 156 7.5. RUS measurement on ScF3 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 158

Ch. 8 : Instrumentation Development . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 164 8.1. Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 164

vii

App. A : Construction of an optical system . . . . . . . . . . . . . . . . . . . . . . . . . . . 186

Bibliography . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

viii

LIST OF FIGURES

1.1.1 (a) The anharmonic potential is shown. The potential is asym- metric, so that increases in temperature (i.e. the amplitude of oscillation of atoms) leads to an increase in the mean interatomic separation, and hence to thermal expansion. (b) The harmonic potential is symmetric and as the temperature is increased the mean separation remains the same hence no thermal expansion . 3

1.2.1 A linear chain of identical atoms. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 1.2.2 Dispersion relation of the 1D chain of atoms. . . . . . . . . . . . . . . . . . . . . 6 1.2.3 A linear chain of two atomic species . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7 1.2.4 Dispersion relation of the 1D chain of two different atoms. . . . . . . . . 9 1.3.1 NTE in ferroelectrics. (a) Unit cell volume of 0.5PbTiO3-0.5(Bi1−xLax)FeO3

(x = 0.0, 0.1, and 0.2) as function of temperature. FE and PE mean ferroelectric and paraelectric, respectively. Taken from [1]. (b) Thermal expansion coefficient of volume in PbTiO3.Taken from [2]. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11

1.3.2 NTE due to valance transitions. (a)Temperature dependence of the unit cell volume of BiNiO3. Low pressure-temperature and high pressure-temperature data are drawn as open and closed circles, and crosses show the weighted average volume in the transition region. From [3]. (b)The dilatometric linear thermal expansion of Bi0.95La0.05NiO3 on heating and cooling showing a 20 K hysteresis. From [3]. (c)Temperature evolution of structure parameter unit cell volume of Sm2.75C60.From[4] . . . . . . . . . . . . . . . 12

1.3.3 NTE in magnetic materials. (a) Temperature dependence of the unit-cell volume of MnF3 . The Neel temperature, TN is shown. From [5]. (b) Relative length changes L/L0 of ferromagnet GdAgMg for various magnetic fields. From [6] . . . . . . . . . . . . . . . . 14

1.3.4 Negative thermal expansion in ZWO. Filled circles represent neu- tron diffraction data while open circle represent dilatometry data. Taken from [7]. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 15

1.4.1 Rotation of 2D perovskite leads to an area reduction. . . . . . . . . . . . . . 20 1.4.2 Representation of the tension effect. A linear linkage of three atoms

is shown in left. This can distort such a way that the central atom displaces transverse direction or the two end atoms displace in opposite ways. In both cases the bonds stay in rigid and the two end atoms move inwards in the vertical direction. Taken from [8] 22

1.6.1 Global structural phase diagram of MF3 type perovskites. . . . . . . . . . 24

ix

1.7.1 Pressure-temperature phase diagram for ScF3. The dashed line is a guide to the eye. Two layers of octahedra in both the cubic and the rhombohedral ReO3 structures (viewed along [111]) are shown. Upon pressurization, octahedral tilts fold the structure so that it is more compact and reduce the symmetry from cubic to rhombohedral. Taken form [9] . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 28

2.1.1 Excitations that may probe using IXS, From [10] . . . . . . . . . . . . . . . . . . 31

2.2.1 X-ray scattering from an arbitrary atoms . . . . . . . . . . . . . . . . . . . . . . . . . 34

2.2.2 Radiation from source (S) to detector (D) via the sample . . . . . . . . . . . 37

2.2.3 Reflection geometry where the blue solid circle represents the jth

atom where −→r j and −→r initiate at the unit cell origin . . . . . . . . . . . . . . 38

2.2.4 Typical features appear on high energy resolution inelastic scatter- ing spectrum . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 50

2.2.5 Phonon creation is shown on left and phonon annihilate process on right . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 51

2.3.1 Simple cubic structure of ScF3 lattice where pink spheres are Sc atoms and orange spheres represent F atoms. From [11] . . . . . . . . . 57

2.3.2 Schematic of IXS spectrometer layout (a) and photograph (b) of the 9 m arm of the spectrometer at sector 30 of APS. The schematic is not to scale. The main components, the direction of incident beam and scattered beam are shown. Sample is mounted on a four circle rotational mount and the detector array is kept as much as close to the sample. Analyzer array is mounted at far end of the arm which is capable of rotate about 32 degrees which is corresponding to maximum of 75 nm−1 momentum transfer. . . . 57

2.3.3 (a) Single crystal ScF3 received from Vladimir Voronov. We named them for identification purpose in future usage. (b) Simple cubic structure formation of ScF3 lattice drawn in to scale where purple spheres are Sc atoms and red spheres represent F atoms. . . . . . . . . 58

2.3.4 (a) Crystal mount used in sector 30 experiment. (b) Dimensions of the crystal Gamma. Crystal sits on wax in order to carry out X-ray diffraction measurement. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 59

2.3.5 Diffraction spots appeared on 2D area detector. Crystal plane is z=o and sample Gamma is used. Lattice planes are shown in dotted lines . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 60

2.3.6 X -ray diffraction data on powder ScF3 sample . . . . . . . . . . . . . . . . . . . 60

x

2.3.7 (a) Mosaic width ∼ 0.0020, as measured on the strong (H,K,L) = (1,1,0) Bragg reflection indexed to the four-atom simple cubic cell (lattice parameter a = 4.016 A at temperature T = 300 K) (b) Lattice volume as a function of temperature determined from tracking the Bragg peak (3,0,0) in single-crystalline ScF3. Inset: The lattice volume over a larger thermal window determined on powder samples[9]. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 61

2.3.8 Overview of the lattice mode dispersion at select momenta and energies. Strong branch softening along the M − R cut is shown by arrows. The longitudinal (LA) and transverse (TA) acoustic branches are shown. Black solid lines are a guide to the eye. Red circles in the inset mark the momenta R + δ (2.39,1.43,0.45) and M + ε (2.39,1.43,0.02) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 62

2.3.9 100 planar section of the octahedra, illustrating the displacement pattern of modes attributed to NTE. The area of the box in (b) is reduced by cos2θ of the area in (a) . . . . . . . . . . . . . . . . . . . . . . . . . . . . 64

2.3.10 First Brillouin zone of simple cubic material ScF3. High symmetry points are shown as well. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 65

2.3.11 (a) The lowest vibrational modes at the M point.(M+ 3 distortion) (b)

The lowest vibrational modes at the R point. The rhombohedral phase can be described as a static tilt according to the R+

4 pattern. 66 2.3.12 (a) Inelastic spectra of SrTiO3 measured at several temperatures.

Left side shows the soft mode behavior and right side shows divergence of central peak. From [12]. (b) Inelastic spectra of SrTiO3 (left) and KMnF3 (right) for approximately equal T=T- Tc. From [12]. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 68

2.3.13 Central peak due to defects and impurities. (a) Integrated central peak intensity of hydrogen reduced SrTiO3 as a funtion of T-Tc [13]. (b) The temperature dependence of the central peak height of the as-grown KH3(SeO3)2 crystal (+) and the crystals used repeatedly (0, ,x)[14] . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 70

2.3.14 Broad and narrow features within the central peak. Solid and dotted curves in (a) represent fitting models, Lorenzian squared

and Lorenzian function respectively[15]. (b) X-ray scans of 1 2

(1,1,5) R point along [0 1 1] direction with 100 keV photon energy beam hitting at the center of the crystal and (c) beam hitting the crystal corner of the crystal. )[16] . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 71

2.3.15 Color maps of the IXS signal at the (a) M (b) R points in reciprocal space . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 73

2.3.16 Color maps of the IXS signal at the (c) M +ε, and (d) R + δ points in reciprocal space. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 73

xi

2.3.17 Resolution convoluted fitting of the IXS data in figure 2.3.16 results in squared mode energies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 74

2.3.18 Resolution convoluted fitting of the IXS data in figure 2.3.16 results in elastic peak intensity. Elastic peak begins to appear near 80 K, which is 120 K above the extrapolated transition temperature. . . . 75

2.3.19 Central peak intensity observed in SrTiO3 [17]. Elastic peak begins to appear 25 K above the transition and the intensity reaches it’s maximum at the transition temperature. . . . . . . . . . . . . . . . . . . . . . . . 75

2.3.20 Cubic and rhombahedral unit cells associated with two phases of transition metal trifluorides other than ScF3 are shown. As shown the rhombahedral phase is associated with rotated ScF6

sub units. Gray circles represent scandium atoms and light blue circles represent fluorine atoms. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 77

2.3.21 Structural phase diagram showing the c-r phase boundary vs the B-site mean radius in 3d transition metal trifluorides and in the solid solutions Sc1xAlxF3 and Sc1xYxF3. Data taken from Refs [18, 19, 20, 21, 22]. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 79

2.3.22 Disorder phase diagram for ScF3. Compositional disorder is quan- tified via the B-site variance σ2

B = rB - rB 2, which has the effect

of increasing the stability of the lowersymmetry, rhombohedral structural phase. Red and orange symbols show the effect of Y and Al substitution, respectively. Dotted lines indicate a linear fit to the Tc(σ2

B), not including the pure sample ScF3. The verti- cal axis intercept reveals a temperature scale ∼ 80-100 K,where central peak elastic scattering and thermal expansion saturation are also observed in pure ScF3 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 81

2.3.23 Transverse vibrations of Fluorine atom . . . . . . . . . . . . . . . . . . . . . . . . . . 82 2.3.24 Acoustic phonon energies along different directions in reciprocal

space. The slope simply gives the acoustic velocities of corre- sponding modes along different directions for ScF3. LA and TA stands for longitudinal acoustics and transverse acoustics respectively . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 83

2.3.25 Poisson ratio obtained from elastic parameters . . . . . . . . . . . . . . . . . . . 85 2.3.26 Youngs modulus obtained using elastic parameters . . . . . . . . . . . . . . . 86 2.3.27 Representative resolution function collected at 6K from plexiglass

co-mounted with the sample . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 88 2.3.28 Schematic of the dynamical structure factor used to fit the data . . . . 89 2.3.29 Sample of fit quality at momentum points R (left column) and M

(right column). The red points and blue lines resemble data and the fit respectively. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 90

2.3.30 Sample of fit quality at momentum points R+δ (left column) and M + ε (right column). . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 91

xii

3.2.1 Structural phase diagrams of (a) 3d transition metal trifluorides and (b) mercurous halides. Insets show the basic volume-defining polyhedral units: (a) the BF6 octahedraon and (b) the elongated square dipyramid (ESD). Development of the structure for (c) the trifluorides and (d) the mercurous halides with the ionic radii indicated as spheres. The basic polyhedral structural unit is superposed in each case. (e) Comparison of the observed bond distances (symbols) and expectations based on hard sphere packing (dashed lines). . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 95

3.2.2 Temperature-dependent lattice parameters of (a,c) ScF3, TiF3, and (b,d,f) Hg2I2, and Hg2Br2. (e) shows a schematic free energy landscape of realized and incipient ferroelastics. Arrows show the fluctuation domain in each case. . . . . . . . . . . . . . . . . . . . . . . . . . . . 96

3.2.3 Rocking curves measured at (330) bragg peak for optical and detec- tor quality Hg2Br2 and Hg2I2 crystals cleaved along 110 planes grown by physical vapor deposition method by Brimrose Tech- nology Cooperation. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 97

3.3.1 Structure of 3d transition metal trifluorides in the (a) high-temperature cubic phase and (b) the low-temperature rhombohedral phase. Structure of the mercurous halides in (c) the high-temperature body-centered tetragonal and (d) low-temperature orthorhom- bic phases. Inelastic X-rays scattering measurement of (e) ScF3

at the simple-cubic R point, corresponding to the soft mode of the rhombohedral transition and (f) Hg2I2 at the BCT X point, corresponding to the soft mode of the orthorhombic transition. Insets show the Brillouin zone in each case. Soft mode frequency squared resultant from fitting to a damped-harmonic oscillator model for (g) ScF3 at R point and (h) Hg2I2 at X point. Dashed lines indicate the extrapolation to negative absolute temperature and indicate the proximity to an incipient ferroelastic transition. . 100

3.3.2 Structure of 3d transition metal trifluorides in the (a) high-temperature cubic phase and (b) the low-temperature rhombohedral phase. Structure of the mercurous halides in (c) the high-temperature body-centered tetragonal and (d) low-temperature orthorhom- bic phases. Inelastic X-rays scattering measurement of (e) ScF3

at the simple-cubic R point, corresponding to the soft mode of the rhombohedral transition and (f) Hg2I2 at the BCT X point, corresponding to the soft mode of the orthorhombic transition. Insets show the Brillouin zone in each case. Soft mode frequency squared resultant from fitting to a damped-harmonic oscillator model for (g) ScF3 at R point and (h) Hg2I2 at X point. Dashed lines indicate the extrapolation to negative absolute temperature and indicate the proximity to an incipient ferroelastic transition. . 103

xiii

4.2.1 Thermal diffuse scattering images of (a) (100) (b) (110) (c) (111) planes taken for ScF3. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 110

4.2.2 Inset: Experimental geometry for the diffuse scattering experi- ments in single-crystal ScF3. Main panel shows a H = 0.5 cross section of the Ewald sphere. Blue and orange arcs indicate the extrema of the crystal rocking angle(1 ) . . . . . . . . . . . . . . . . . . . . . . . 112

4.2.3 (a) Diffuse scattering intensity collected using the experimental geometry in Figure 4.2.2. Mid-zone intensity at M points are indicated by dashed circles and are found in almost every BZ. Dashed lines indicate cuts through the intensity patterns shown in (b). Each cut in (a) is taken an an equivalent K value but corresponds to a different L value. The negligible change in widths is strong evidence of 2D spatial correlations. . . . . . . . . . . . . 113

5.1.1 (a) A 5 × 5 × 5 crystallite of ScF3 in the average structure (125 octahedra). (b) The hollow cube shows the simple cubic BZ with shaded regions indicating the positions of observed scattering rods from the data in Figure 4.2.3. Breakouts show possible real- space staggered rotation patterns which preserve internal octa- hedral dimensions at the indicated high-symmetry momentum- space points. Red and blue shading in the diamonds indicate equal but opposite magnitudes of rotation. . . . . . . . . . . . . . . . . . . . . . 115

5.1.2 A model consisting of stiff diamonds connected by hinged joints shown. As a result of the constraints, a staggered rotation by an angle θ in (b) causes a shortening of the vector locating each diamond by a factor cos θ . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 116

5.2.1 (a)(d) show classical solutions for θ(t) which follow from Equation 5.2.3. These are plotted for different values of k0, which uniquely quantifies the anharmonic behavior. The time axes in (a) and (c) are scaled by the FM period . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 120

5.3.1 (a) Lattice parameter of ScF3 below T = 300 K from Ref. [23] (b) Transverse fluorine thermal parameter determined from x- ray pair density function analysis [18]. Superimposed on (a) and (b) are the corresponding quantities from (2) using Nx = 5.5 for varying values of ~ωp (c) Velocity field superimposed on a homogeneously excited FM, with phase and kinetic energy below. (d) shows the significant kinetic energy lowering when a π/2 defect is introduced. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 123

6.4.1 A sample spectra taken for ScF3. The frequency-dependent optical behavior of ScF3 is divided in regions: T for transmission (or ”transparency”), A for absorption and R for reflection. . . . . . . . . . . 132

xiv

6.4.2 Compare the parameters obtained from factorized form model and Lorentzian model. Black markers are obtained from lorentzian model and colored plots are from factorized form model. . . . . . . . . 133

6.5.1 Gray sphere represents Sc atom while Blue spheres represent F atoms. Black arrows show the direction of displacement. (a) Acoustic mode. (b) The lowest energy optical mode. This is also known as silent mode (c) The highest energy mode (TO2 in our case) (d) The low energy mode which is also known as breathing mode.(TO1 in our case) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 134

6.6.1 Measured reflectance of ScF3 sample at different temperatures . . . . . 135 6.6.2 (a),(c) TO phonon energies & (b),(d) LO phonon energies obtained

for ScF3 by fitting the reflection with factorized formula at dif- ferent temperatures. Corresponding linewidths obtained are shown in insets . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 138

6.6.3 (a) Temperature dependance of imaginary part of permitivity ,Imε(ω). Peak values are corresponding to TO phonon peaks. The inset shows the resulted peak due to two phonon scattering. The In- set scale is magnified by 100. (b) Temperature dependance of loss function,-1/Imε(ω). Peak values are corresponding to LO phonon peaks. The inset shows the resulted peak due to two phonon scattering. Inset scale is magnified by 100 . . . . . . . . . . . . . . 139

6.6.4 Variation of the real part of the dielectric function for ScF3 with temperature. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 140

6.6.5 Most probable combination of two phonons are shown. They could be arising from sharp DOS which is shown in extended blue area in combined plots of phonon dispersion and corre- sponding DOS. Directions along Γ - M - R and along Γ - X - M are considered. A mode lies at momentum point -q with in red( at momentum point q in green) areas of dispersion plot corresponding to higher energy DOS peak and a mode lies at momentum point q with in red( at momentum point -q in green) areas in the lower energy DOS peak excite and correspond to two phonon absorption. Dispersion plots are taken from [24] . . . . 145

7.2.1 Stress tensor components acting on a body with respect to a three- dimensional Cartesian coordinate system . . . . . . . . . . . . . . . . . . . . . 151

7.2.2 Information hidden in elastic stiffness tensor elements are shown in matrix form for clear view . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 152

7.3.1 Typical setup used for RUS measurements . . . . . . . . . . . . . . . . . . . . . . . 155 7.4.1 (a) Single crystal ScF3 used for RUS measurement. This is the

second shipment of crystal received from Vladimir Voronov. (b) Experimental setup used in Los Alamos National Laboratory . . . . 157

xv

7.5.1 Typical example of RUS signal. Two sharp peaks indicate reso- nance vibrations of ScF3 lattice around 500 kHz . . . . . . . . . . . . . . . . 159

7.5.2 Resonance vibrations around 600 kHz . . . . . . . . . . . . . . . . . . . . . . . . . . . 159 7.5.3 Temperature dependence resonance(around 775 kHz) for crystal

ScF3. Red line indicates the energy dissipation or the width of the resonance peak as a function of temperature . . . . . . . . . . . . . . . . 161

7.5.4 Temperature dependence resonance(around 380 kHz) for crystal ScF3. Red line indicates the energy dissipation or the width of the resonance peak as a function of temperature . . . . . . . . . . . . . . . . 162

8.2.1 Spherical mirror wouldn’t be the best choice when the object and the image is non collinear . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 167

8.2.2 Prolate ellipsoid with two planes of interests. Two planes are orthoganal to each other. Unit vector represents the center of the to be constructed mirror. Two orthogonal ROCs are given by the projections of the planes on the ellipsoids . . . . . . . . . . . . . . . . . . . . . . 169

8.2.3 Prolate ellipsoid with focii at(−d, 0, 0) and (d, 0, 0). (x0, 0, z0) denotes the center position of the to be constructed mirror with specifica- tions s, t and α. They denote the object distance, image distance and the angle in between respectively. . . . . . . . . . . . . . . . . . . . . . . . . . 170

8.2.4 Exact surface in which the mirror is grinded is the ellipsoidal shape shown in green. But in our design process we used toroidal surface shown in red as an approximations to the ellipsoidal shape. The point of interest in which the two orthogonal ROC were calculated is (x0, 0, z0). Orange bordering around the point of interest approximately represents the mirror surface obtained. . 171

8.2.5 Optical layout combined with cryocooler. Specifications of each mirrors are given in Table 6.1. Gray colored mirrors are plane mirrors and the whole layout can be rotated around them. A sharp aperture is placed at the focus of M0 mirror. This defines the object to M1 mirror which forms an image at the sample space. Light reflects from and transmits through the sample are collected by M2r and M2t mirrors and refocused into detec- tors(Red colored) by M3r and M3t mirrors . . . . . . . . . . . . . . . . . . . . . . 172

8.2.6 Custom made components for optical cryocooler. . . . . . . . . . . . . . . . . 174 8.3.1 THz frequency range with respect to the whole electromagntic

spectrum. The range approximately is in between 2 meV and 20 meV. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 176

8.3.2 Current THz spectrometer. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 179 8.3.3 Comparison between electro-optic detection and antenna detection

setups . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 180 8.3.4 The virtual source point for the BATOP antenna is roughly = L - d

= 18.7 mm behind the antenna chip . . . . . . . . . . . . . . . . . . . . . . . . . . . 182

xvi

8.3.5 Time Domain THz signal . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 185 8.3.6 Frequency Domain THz signal . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 185

A.3.7 ellipse shown in xyz coordinate,y is perpendicular to the plane . . . . 186 A.3.8 two coordinate systems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 190 A.3.9 ellipse representing in two coordinates . . . . . . . . . . . . . . . . . . . . . . . . . . 191

xvii

LIST OF TABLES

2.1.1 List of techniques broadly grouped under the heading of Inelastic X-Ray Scattering.From[10] . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 32

2.3.2 Summary of elastic properties of similar type of materials. Bulk modulus (B), Shear modulus (G) and Zener anisotropy (A) are shown as well . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 84

6.6.3 Compare the fit models at 300 K. Unites are given in cm−1 . . . . . . . . . 136 6.6.4 Comparison of our experimental results with previous calculations

at 300 K. Units of energies are cm−1. . . . . . . . . . . . . . . . . . . . . . . . . . . . 137 6.6.5 Static dielectric constant for ScF3 obtained from LST relation . . . . . . . 143 6.6.6 Two phonon absorption possibilities, if only high symmetric points

are considered . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 144

8.2.7 Specifications of mirrors used in mirror layout shown in Figure 8.2.5. Here∞means the beam is parallel. The mirror notation is used for identification purpose. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 173

xviii

1.1 Thermal expansion

Materials tendency to decrease or increase their volume when heated is known

as thermal expansion. The vast majority of materials increase in dimension

when they are heated corresponding to positive thermal expansion (PTE).

While thermal expansion is common among all three phases of substances, in

solids it may be isotropic or anisotropic. Substances expand in same amounts

along any direction known as isotropic expansion, which is different from

anisotropic case where materials expand in different amounts along different

crystallographic orientations.

Thermal expansion in solids is a direct consequence of the anharmonic nature

of interatomic forces between atoms (anharmonic potential) (Figure 1.1.1a).

The mean separation between atoms correspond to the minimum potential is

identified as the equilibrium distance between them. As the temperature is

increased the potential energy of the system increases and the asymmetry of

potential suggests an increase in mean separation, hence thermal expansion.

On the other hand if the atoms behave in harmonic manner, then the mean

1

separation between atoms would not change even the vibrational amplitude

increases with increasing temperature, hence no thermal expansion (Figure

1.1.1b).

Thermal expansion is typically quantified by using coefficient of thermal expan-

sion(CTE), which simply is the relative change in material dimension within

a given change in temperature at constant pressure. In order to measure

the relative change along a certain directions in a solid object, the linear

CTE, αL = (1/L)(∂L/(∂T)P, is defined and this is frequently used to quantify

anisotropic thermal expansion. The magnitude of the thermal expansion is

mostly expressed in terms of volumeteric CTE, αV = (1/V)(∂V/(∂T)P where V is

volume, T is temperature and P is pressure. The CTEs is expressed in unit K−1

and for solids in general the CTEs are of the order of 10−6 and the unit ppm/K

is used instead.

1.2 Lattice Dynamics

Lattice dynamics is the study of vibrations of the atoms in a crystal. It is an

important phenomenon to understand and governs the key properties of mate-

rials such as thermodynamics, phase transition, thermal conductivity, thermal

expansion, and sound wave propagation. More importantly it interacts with

electromagnetic radiation. In lattice dynamics study the atomic motions are

described by traveling waves. Each wave is characterized by wavelength λ,

angular frequency ω, amplitude and direction of travel. For the convenience

2

Figure 1.1.1: (a) The anharmonic potential is shown. The potential is asymmet- ric, so that increases in temperature (i.e. the amplitude of oscillation of atoms) leads to an increase in the mean interatomic separation, and hence to thermal expansion. (b) The harmonic potential is symmetric and as the temperature is increased the mean separation remains the same hence no thermal expansion

wavelength is being replaced with wave vector k= 2π/λ.

Simplest form of lattice dynamics theory uses harmonic approximation. Con-

sidering the potential given in Figure 1.1.1a the Taylor series expansion around

equilibrium distance between atoms, r0 can be written as

V(r) = V0 + 1 2 ∂2V ∂r2 (r − r0)2 +

1 3! ∂3V ∂r3 (r − r0)3 +

1 4! ∂4V ∂r4 (r − r0)4 + .... (1.2.1)

In harmonic approximation only the quadratic terms is retained. In most cases,

the approximation is very effective and if not, we can start with it and then

modify the model by adding higher order terms for better results of inter-

3

atomic forces, wave vectors and frequencies. Nevertheless, properties such

as thermal conductivity, thermal expansion, and phase transition can not be

explained by the harmonic model.

Consider a crystal with one atom per unit cell, as an example, a 1D chain of

atom, each of mass m. The atoms are connected by elastic springs, so the force

between the atoms are directly proportional to relative displacement from the

equilibrium position. Let us assume that the separation between consecutive

atoms is a, so the position of the nth atom in 1D chain is na (Figure 1.2.1). We

define the displacement of nth atom to be Un and write equation of motion of

an atom

Fn = C((Un+1 −Un) − (Un −Un−1)) = m d2Un

dt2 (1.2.2)

where C is the force constant.

For any coupled system, a normal mode is defined to be a collective oscillation

where all particles move at the same frequency. Let us now attempt a solution

4

Un = U0ei(ωt−kna) (1.2.3)

where U0 is the amplitude of oscillation and k is the wave vector.

Plugging the solution to Equation 1.2.2 we get

−mω2U0ei(ωt−kna) = CU0eiωt[e−ika(n+1) + e−ika(n−1) − 2e−ikan] (1.2.4)

mω2 = 2C[1 − cos(ka)] = 4C sin2(ka/2) (1.2.5)

and we obtain the result

ω = 2

√ C m

sin (ka

2

). (1.2.6)

The relationship, ω(k) is known as the dispersion relationship of the correspond-

ing atomic structure. Figure 1.2.1 shows the dispersion relation and it is pe-

riodic in k → k + 2π/a. Following this we use the term k-space which is also

known as reciprocal space. The periodic unit in reciprocal space is known as Bril-

louin Zone(BZ) and Figure 1.2.1 shows only the ”First Brillouin Zone” which

has the boundaries at k= ±π/a.

5

Figure 1.2.2: Dispersion relation of the 1D chain of atoms.

One important consequence of dispersion relationship in 1D chain is that it

allows us to calculate group velocity, Vg = dω/dk and phase velocity, Vp =

ω/k. With the particular dispersion relation given in Equation 1.2.6 the group

velocity

Vg = 2(Ca2/m)1/2 cos(ka/2). (1.2.7)

In long wavelength limit, where cos ka ∼ 1-(ka/2)2, the dispersion relation be-

comes

ω2 = (C/m)(k2a2) (1.2.8)

and we obtain a result that the velocity in long wave length limit is independent

6

of frequency. Recalling that the sound wave is a vibration that has long wave

lengths, we obtain the result

Vsound = a

√ C m . (1.2.9)

We discussed a classical system which has normal mode of frequency ω. The

corresponding quantum mechanical system will have eigenstates with energy

En = ~ω(n + 1 2

) (1.2.10)

which the energy of a lattice vibrations is quantized and quantum of energy

is called Phonon. This is analogues to quantized energy called photons of the

electromagnetic wave.

We now extend the discussion to analyze linear chain with two atomic species

(Figure 1.2.3). Writing down equations of motions

Figure 1.2.3: A linear chain of two atomic species

7

dt2 (1.2.11)

dt2 (1.2.12)

Un = U0ei(ωt−kna) (1.2.13)

Vn = V0ei(ωt−kna) (1.2.14)

(C1 + C2eika)U0 + (mω2 − C1 − C2)U0 = 0 (1.2.16)

where for simplicity here we used m1=m2.

The solutions to this are obtained by finding the zeros of secular determinant (mω2

− C1 − C2) (C1 + C2e−ika)

(C1 + C2eika) (mω2 − C1 − C2)

= 0

8

1 + C2 2 + 2C1C2 cos(ka). (1.2.17)

Figure 1.2.4: Dispersion relation of the 1D chain of two different atoms.

This method can be generalized for more complex three-dimensional materials

and most of the advanced condensed matter textbooks explain this approach

thoroughly. To complete the normal mode solution in three dimensional, the

vibrational amplitude should be incorporated which can be used to calculate

the total energy of the crystal as well.

1.3 Negative thermal expansion

It is not uncommon that some materials show the opposite behavior of PTE,

9

which they shrink upon heating give rise to negative thermal expansion (NTE).

This is relatively new filed of study, yet we have seen phenomenal development

in recent years as many materials are discovered displaying this unusual be-

havior. The most popular example for NTE phenomenon is the liquid water-ice

expansion below 40 C and above ice-water phase boundary.

Even though not all of the different mechanisms responsible for NTE are fully

understood, generally the origin of NTE is viewed in two different ways. NTE

could either arise from non-vibrational effect associated with electronic and

magnetic instabilities or emerge from vibrational effect associated with intrinsic

geometrical instabilities.

1.3.1 Negative thermal expansion from phase competition

The non-vibrational effects account for NTE are mostly related with phase

transitions and one of the very well known example for this type of materials

family is ferroelectrics. Interestingly, some ferroelectrics exhibit NTE or anoma-

lous thermal expansion properties below the curie temperatures and their NTE

originates from ferroelectric order which occurs due to the strong hybridization

between cations and anions. Some of the notable examples in this category are

PbTiO3[2, 25, 26, 27],PbTiO3 based compounds[28, 1], BaTiO3[29], BiFeO3[25],

Pb(Zn1/3Nb2/3)O3[30], Ca3Mn2O7[31], Ca3Ti2O7[31] and Sn2P2S6[32]. The NTE

associated with the spontaneous polarization originating from Pb/Bi-O hy-

bridization is reported for PbTiO3-based compounds [28] and they have at-

10

tracted attention due to the precise capability of controlling NTE, not just in

a single way but by using various methods such as the chemical modifica-

tion, size effect, and physically by applying pressure. A couple of examples of

ferroelectric NTE are shown in Figure 1.3.1.

Figure 1.3.1: NTE in ferroelectrics. (a) Unit cell volume of 0.5PbTiO3- 0.5(Bi1−xLax)FeO3 (x = 0.0, 0.1, and 0.2) as function of temperature. FE and PE mean ferroelectric and paraelectric, respectively. Taken from [1]. (b) Ther- mal expansion coefficient of volume in PbTiO3.Taken from [2].

The change of electron configuration can also cause NTE and abnormal thermal

expansion properties to some materials. The volume increment upon cooling

due to a valance transition has been reported for rare earth fulleride Sm2.75C60

[4]. NTE in BiNiO3 [3] is attributed to atomic radius contraction caused by

intermetallic charge transfer from Ni to Bi. Others display NTE due to intersite

charge transfer, as reported in perovskites oxides such as SrCu3Fe4O12[33] and

LaCu3Fe4O12[34]. Even semiconductors (e.g. Si, Ge, and GaAs [35, 36]), su-

perconductors (e.g. MgB2, Ba(Fe0.926Co0.074)2As2 [37, 38]) and Mott insulators

(e.g. Ca2RuO4 based compounds [39, 40] ) exhibit NTE or anomalous thermal

11

expansion properties as a result of change in electron configuration. There exist

a number of ways to tune NTE due to phase competition, including controlling

free electron concentration of semiconductors, modulating the metal insulator

transition of Mott insulator, and introducing quenched disorder. An attribute

of this approach is the potentially large CTE, although a drawback in most

cases is persistence over only a narrow temperature range.

Figure 1.3.2: NTE due to valance transitions. (a)Temperature dependence of the unit cell volume of BiNiO3. Low pressure-temperature and high pressure- temperature data are drawn as open and closed circles, and crosses show the weighted average volume in the transition region. From [3]. (b)The dilatomet- ric linear thermal expansion of Bi0.95La0.05NiO3 on heating and cooling showing a 20 K hysteresis. From [3]. (c)Temperature evolution of structure parameter unit cell volume of Sm2.75C60.From[4]

A change in volume in response to staggered or uniform spontaneous magneti-

12

zation is known as magnetovolume effect” has been identified as the cause for

anomalous thermal expansion of magnetic materials. The underlying nature

of NTE or anomalous thermal expansion in magnetic materials is the coupling

between magnetic order and the lattice. The first discovery of low thermal

expansion material of this type happened to be in 1897 by Guillaume and it

was the famous industrial alloy InVar (Fe.64Ni.36) [41]. Since then there are

many known magnetic materials which exhibit NTE include alloys (GdAgMg

[6] ), iron based alloys ( Nd2Fe17Nx[42], Gd2Fe17[43]), oxides ( (La0.8Ba0.2)MnO3

[44]), sulphides(CdCr2S4 [45]), fluorides (perovskite MnF3 [5] ) and nitrides

(antiperovskite manganese alloy based nitrides [46]). These materials display

a variety of unusual mechanical properties such as large, tunable CTE over

a considerable temperature span. An excellent review of NTE in functional

materials can be found in literature [47]

1.3.2 Negative thermal expansion from framework dynamics

Besides NTE from phase competition, there also exists a growing class of mate-

rials with strong, isotropic, robust and thermally persistent NTE that originates

from vibrational mechanism, or in other words intrinsic structural degrees of

freedom. NTE of this type has recently been described as structural negative

thermal expansion (SNTE) [48].

SNTE is a fascinating and growing field of condensed matter physics due

to the rarity of the phenomenon, stunning display of unconventional lattice

13

Figure 1.3.3: NTE in magnetic materials. (a) Temperature dependence of the unit-cell volume of MnF3 . The Neel temperature, TN is shown. From [5]. (b) Relative length changes L/L0 of ferromagnet GdAgMg for various magnetic fields. From [6]

dynamics, and strong potential for structural applications where dimensional

stability is required. This type of NTE phenomenon refers to the unusual

tendency for materials to shrink when heated as a property of bond network

topology and the associated fluctuations [49, 50, 51] which is distinct from NTE

arising from electronic or magnetic degrees of freedom described in section

1.3.1.

SNTE is most often discussed in connection with transverse fluctuations of

a linkage between volume defining vertices, which may accompany the libra-

tional (rocking) vibrations in rigid bonds or hindered rotational motion of rigid

polyhedral subunits. The most studied example that shows this type of be-

havior is ZrW2O8 (ZWO) [7, 52, 53, 54, 55, 56]. This cubic material has a large

unit cell, containing 44 atoms in the form of corner linked ZrO6 octahedra and

14

Figure 1.3.4: Negative thermal expansion in ZWO. Filled circles represent neutron diffraction data while open circle represent dilatometry data. Taken from [7].

WO4 tetrahedra. The NTE behavior is strong (Figure 2.3.9) in ZWO ( αV = -27.3

x 10−6/K up to 400K) compared to most of NTE materials of this class and re-

ported over wide range of temperature range (0.3-1050 K). The ZrO6 octahedra

and WO4 tetrahedra connect via the corner O atom, but one of the O in WO4 is

not connected to another unit and the origin of the NTE comes from transverse

vibration of Zr - O - W bond [57]. At the same time, the NTE in ZWO survives

even after a phase transition occurs at 430 K, but the volumetric thermal expan-

sion coefficient decreases to -18 x 10−6/K. Well-known categories of materials in

which the NTE behavior has been attributed to vibrational mechanisms include

metal cyanides [58], various zeolite frameworks [59], A2M3O12 series [60, 61],

ZWO family[7, 62], ZrV2O7 family[63, 64], Prussian blue analogues[65], MOF-5

materials [66, 67] and metal fluorides [68].

15

1.4.1 Grneisen theory and thermal expansion

As introduced by Germen Physicist Eduard Grneisen [69, 70], Grneisen theory

assumes that the phonon frequencies of a crystal are modified as the volume

changes. The changing frequencies would allow calculating thermodynamic

functions with in harmonic approximation. This approach is known as quasi-

harmonic approximation. See reference [71] for more details.

Within Grneisen theory, for a crystal with many normal modes, the mode

Grneisen parameter is defined, which explains the effect that changing the vol-

ume of a crystal lattice has on its vibrational properties, and as a consequence,

the effect that changing temperature has on the size or dynamics of the lattice.

Since thermal expansion is a result of the anharmonic nature of bonds, quan-

tification of the anharmonicity in a solid can be achieved with mode Grneisen

parameter, γ(q)i. The mode-dependent Grneisen parameter for a phonon mode

i at a reciprocal lattice point q can be defined as

γ(q)i = − ∂ logω(q)i

∂ log V (1.4.1)

where V is the unit cell volume, and ω(q)i is the frequency of the ith mode of

vibration, which itself is a function of a wave vector q in the BZ.

Equation 1.4.1 implies that for a NTE material, γ(q)i is negative, for modes

16

soften with increasing temperature and positive, for modes stiffen with in-

creasing temperature. The overall expansion behavior of a material depends

on the combined contributions from all modes, therefore materials with neg-

ative mode Grneisen parameters are not necessarily NTE materials. Often

thermal expansion is quantified by mean Grneisen parameter, obtained by

integrating Equation 1.4.1 over all modes:

γ = − αVBV

CV (1.4.2)

where B is bulk modulus and CV is constant volume heat capacity. As B,CV,

and V are positive for materials in thermodynamic equilibrium, NTE materials

necessarily possess a negative mean Grneisen parameter.

1.4.2 Rigid unit mode picture

Studies have shown that the lattice vibrations responsible for NTE in ZWO

are in the energy scale of around 2 meV [55, 50, 72, 73]. The bond stretching

and bond bending modes are mostly frozen at this energy scale and vibrations

which respect and maintain internal polyhedral distances and bond angles

have special significance. The WO4 tetrahedral stretching and bending modes

are not thermally excited at the low temperatures where NTE begins, [56]

suggesting a hierarchy of energy scales: stiff bond stretching, intermediate

bond bending, and a set of low- energy external modes of rigid polyhedra

17

units called rigid unit modes (RUMs). The latter set may be supported at low-

energy only in certain regions of reciprocal space which are particular to the

system under consideration.

The RUM model was first used to explain the displacive phase transitions in

silicates [74, 75]. It was developed to describe the behavior of materials with

crystal structures that can be described as frameworks of linked polyhedra

(examples are ScF6 octahedra in ScF3 and WO4 tetrahedra in ZWO). Vallade

and coworkers [76] have shown that the softening of an optical mode nearby

an acoustic phonon causes the phase transition of the material quartz and the

whole phonon branch has a low frequency at each k values, hence must be

associated with RUMs not only at one k value, but along the whole branch.

The idea of RUMs acting as soft modes for displacive phase transition was

later developed for silicates using a split atom method.

The RUM model has given a number of other new insights and most impor-

tantly it has also been used to explain the origin of negative thermal expansion

in framework structures. Phonons described by RUM model are associated

with collective motion of polyhedra and those collective motions cause atomic

displacement without distorting the polyhedra. Therefore these modes are

often identified as NTE modes in SNTE materials. Usually the polyhedra vi-

brational energies are very high when they are distorted compared with the

energy when they are not distorted. As a result, we generally expect RUM

modes to have low energies. For ZWO the manifold of momenta supporting

18

RUMs is very complex, as identified through classical calculations [54] using

split atom approach. Simplest case of RUMs associated NTE is described in

cubic lattice systems ScF3 and ReO3 and more importantly their RUMs corre-

spond to simple momentum space manifolds. ScF3 has only four atoms per

unit cell and forms with corner linked octrahedra of ScF6. High symmetry

points of Brillouin zone (BZ), corresponds to in phase rotation of each stack of

octrahedra (M point) and out of phase rotation of each stack of octrahedra (R

point) defines the boundaries of RUM in ScF3 material. Please see Figure 5.1.1

for a better view on this.

Welches and coworkers have developed a simple qualitative picture explaining

NTE [77] in ReO3 like structures. It is related with geometrical frame work and

is associated with the rotation of stiff structural units or bond bending of the

shared corner atom of the polyhedra units by preserving the rigid unit structure

(RUM). For simplicity the rotation of a 2D perovskite (2D frame work of linked

squares) is considered and the important point is that the area or lattice constant

is reduced by the rotation as a straightforward geometrical effect(Figure 1.4.1).

Considering the potential energy of rotation due to thermal fluctuations, 1 2

Iω2 θ2 T =

1 2

kBT2 where I is the moment of inertia of the units, ω2 is average or Einstein

frequency for the rotations, θ2 T is the equilibrium fluctuating value of θ2 at

temperature T, kB is Boltzmanns constant. Considering the lattice area reduc-

tion, from A0 to A0 cos2 θ the lattice constant obeys the relation a = a0(1 − ηaθ2)

and the expression a a

= − ηakBT Iω2 is obtained, which then reduces to CTE

19

Figure 1.4.1: Rotation of 2D perovskite leads to an area reduction.

αL = − ηakB

Iω2 . Here ηa is identified as geometrical constant which is equal to

unity in this case. Chapter 5 discusses a model that we developed to approx-

imate the staggered rotation in 2D square lattice and proves that the above

constant equals to 1/2 in a 2D lattice with few squares, where harmonic wave

limit is applied and 2/3 in a lattice with large number of square units, where

circle wave limit is applied.

As shown the geometrical effect on the CTE leads to a negative CTE. At the

same time since the frequency of modes appears at the bottom of the CTE it

resembles that the softer modes contribute more to the CTE. A particularly

soft dynamic distortion of this structure preserves bond lengths and internal

polyhedral bond angles while decreasing the volume of the time-averaged

structure as the vibrational amplitude is increased through thermal activation.

This classical picture has been widely discussed in general reviews of the NTE

20

phenomenon[78, 79, 80, 81].

1.4.3 Tension effect and NTE

SNTE is commonly described using a mechanism called tension effect which is

thoroughly discussed in the review [8]. The simplest form of the tension effect

considers a linear molecule which consists of three atoms. As the center atom

of the linkage move transversely, the corner atoms move towards each other,

assuming the bonds are rigid. Applying this into three dimensional (3D) struc-

ture immediately implies that the structure decreases it’s dimensions, hence

NTE. As the corner atoms of the linkage move further away from each other

the amplitude of the transverse fluctuation of the center atom decreases and

results in increasing volume. This results in increasing stretch or the tensions

of the bonds, suggesting negative Grneisen parameter. Thermal ellipsoids dis-

played by 3D systems such as ScF3 and ReO3 are consistent with the tension

effect and the mechanism is most useful in interpreting the NTE of CN− frame-

work structures such as AgCN, AuCN, CuCN and Ni(CN)2. RUM model is a

special case discussed under tension effect.

1.4.4 Thermodynamics of NTE materials

A study [82] has shown that for materials with positive compressibility and

NTE, the first law of thermodynamics reads as dQ = dU−PdV. The author has

mathematically proved, that the first law of thermodynamics (dQ = dU + PdV)

holds true only if either both the compressibility and thermal expansion are

21

Figure 1.4.2: Representation of the tension effect. A linear linkage of three atoms is shown in left. This can distort such a way that the central atom displaces transverse direction or the two end atoms displace in opposite ways. In both cases the bonds stay in rigid and the two end atoms move inwards in the vertical direction. Taken from [8]

negative or both of them are positive. A different [83] study has proposed

the isentropic (constant entropy) volume expansivity, αV = (1/V)(∂V/(∂T)S

for materials with NTE instead of standard definition of isobaric (constant

pressure) CTE, αV = (1/V)(∂V/(∂T)P.

There are plenty of materials found to be possessing NTE property and thou-

sands of literature have been published directly or indirectly related with NTE

phenomenon, but only a handful numbers of thermodynamic analysis on NTE

materials are found in literature. So readers who are interested would find it

is worth working in this field.

1.5 Perovskites

22

Perovskite oxides, a class of solid materials with chemical formula ABO3, con-

tains examples of perhaps every possible type of material behavior. Underpin-

ning the competing interactions behind this diversity are fascinating cascades

of structural transitions associated with tilts of the BO6 octahedra, which are

strongly influenced by the A-site ions through geometric tolerances[84, 85].

A-site-free perovskites based on oxygen are rare, as the B ion must take on the

extremal +6 valence state, and the only known instance is ReO3. A moderately-

sized NTE effect occurs at low temperature in this material[86] and can be

understood in terms of a model of rigid unit modes (RUMs) described in sec-

tion 1.4.2. Though that is the case with oxides, A site free perovskite fluorides

or in other words MF3-type structures are not rare because of the common

trivalent(+3) state found in most of the metals in the periodic table, especially

among transition metals and lanthenides.

1.6 Trifluorides and their structures

Figure 1.6.1 shows a global structural phase diagram of MF3 perovskites, where

M is a +3 metal ion. For large (rS > 0.85A) ionic radius rS (Shannon), fluorine

ions can pack around the M ion with high F coordination up to n=8 or 9 in com-

mon large-gap optical materials of orthorhombic and tysonite type structures

which are commonly formed with rare earth metal ions.

Order-disorder type second order phase transitions has been reported for LaF3

- NdF3[87] (refer Figure 1.6.1), from low temperature trigonal(P3c1) to high

23

Figure 1.6.1: Global structural phase diagram of MF3 type perovskites.

temperature hexagonal (P63/mmc) phases which both are two modifications

of tysonite type structure[88]. SmF3 - GdF3 crystallize from melt to tysonite

type structure and upon cooling they transform into orthorhombic(Pnma) β-

YF3 [89] type structure. Structural phase transitions occurred in TbF3, DyF3

and HoF3 are accounted for some sort of impurity[90, 91, 92] in the system and

no transition has been reported for pure systems. ErF3 - YbF3, LuF3 and YF3

yield a new high temperature form of α-YF3 type[92].

Below rS < 0.8A, perovskites form with simple-cubic symmetry(Pm3m) at high

temperatures. At low rS, and among the 3d metal trifluorides, a structural

cubic-to-rhombohedral(R3c) phase boundary is apparent, with the exception

24

of MnF3. ScF3 is the only trifluoride with cubic symmetry at room temperature

and can be considered to be the standout among all and will be discussed

thoroughly through out the thesis.

1.7 Scandium trifluoride(ScF3)

Recently, nonmagnetic ionic insulator ScF3 has drawn particularly intense at-

tention in the chemistry community[9] as the first instance of a perovskite-

structured material with strong, isotropic, and thermally persistent NTE, a

distinction which no longer appears to be an isolated case[93]. ScF3 displays

strong NTE (-42 ppm/K < αV < 0) over a temperature window of 1000 K, but is

also unusual in its lack of any type of phase transition whatsoever within the

solid state.

Cubic ScF3 has 4 atoms per unit cell and consists of corner-inked octahedra

which fill space in three dimensions with unit cells a = b = c. The high

symmetry points in the first Brillouin zone (BZ) in reciprocal space are labeled

zone center Γ(0, 0, 0), zone face center X (2π/a(1/2, 0, 0)), zone edge center

M(2π/a(1/2, 1/2, 0)), and zone corner R(2π/a(1/2, 1/2, 1/2)). Sc has the longest

Shannon effective ionic radius of all 3d transition metal trifluorides, and the

lattice dimension parameter a = 4.02 Å at room temperature is very close to

twice the sum of these radii for Sc (0.745 ) and F (1.19 Å), suggesting chemical

25

1.7.2 Pressure induced phase transition in ScF3

Cubic ScF3 further stands out among substances in that it has the most stable

structural phase of any known solid trifluoride, retaining cubic symmetry from

its high melting point >1800 K to <0.5 K[9, 94]. A finite-temperature cubic to

rhombohedral (c-r) transition can be induced however through application of

slight pressure [95, 96] (<0.2 GPa ∼ 2000 atm), chemical substitution of Ti[20],

Al[19], or Y[97] for Sc, and even by the weak stresses induced by polymeric

impregnation of powder samples[21], suggesting that the quantum nature of

the cubic phase at low temperature is delicate and susceptible to even mild

perturbations.

X-ray diffraction [95, 9] and Raman spectroscopy[95] results have revealed

that at room temperature ScF3 undergoes a pressure induced phase transition

from c-r between 0.5 and 0.8 GPa and rhombohedral to orthorhombic structure

above 3.0 GPa. As suggested by the authors[95] the first transition point which

is quite low as hydrostatic pressure is the result of disturbance of the balance

between short-range dipoledipole(of fluorine ions) and long-range Coulomb

interactions which is related to rotation of the ScF6 octahedra around a threefold

axis. The rotation of octahedra corresponds to R = π/a(1, 1, 1) point in cubic

phase BZ and the c-r phase transition occurs due to condensation of this mode

(Figure 1.7.1).

Observed pressure dependence of the transition temperature is dTc/dp ∼ 525

K/GPa [9, 95, 96]. The c-r phase transition in ScF3 is never realized down to 0.4

K [94] in atmospheric pressure and using inelastic x-ray scattering (Chapter:2)

results, we estimate that pressures as small as 740 bar = 0.074 GPa would be

sufficient to drive the transition upward to 0 K. The sensitivity of the phase

boundary suggests that the nature of the cubic phase is delicate at low temper-

ature and susceptible to even mild perturbations [21, 20, 20, 19]. Section 2.3.10

further discusses this.

If suitable substrates of ScF3 are developed, new functionalities may be reached

in film synthesis, as cooling from the growth temperature would effectively

stretch epitaxial films. Significant efforts in the physics groups of Profs. Barrett

Wells in Physics Department have already produced thin films of NTE ScF3

[98]. Thin films of ScF3 are grown using pulsed laser deposition, and while

large fraction of a film is having very good epitaxy and small mosaic, remaining

regions are polycrystalline. Unique features of this material such as large band

gap, non-oxide nature, poor adhesion under pressure and high saturated vapor

pressure remain as significant challenges to overcome.

1.7.3 Electronic structure of ScF3

In formation of ScF3, from a scandium atom and a fluorine atom, the scandium

atom loses its three valence electrons (and turn to Sc+3 ) to three fluorine atoms

(and form F−), which each of the fluorine has just enough space to accept it. We

27

Figure 1.7.1: Pressure-temperature phase diagram for ScF3. The dashed line is a guide to the eye. Two layers of octahedra in both the cubic and the rhombo- hedral ReO3 structures (viewed along [111]) are shown. Upon pressurization, octahedral tilts fold the structure so that it is more compact and reduce the symmetry from cubic to rhombohedral. Taken form [9]

must realize that unlike other 3d type transition metal trifluorides Sc+3 in ScF3

has 1s2 2s2 2p6 3s2 3p6 4s2 3d0 configuration and hence no free d electrons. One

consequence is that ScF3 has no local moment magnetism and no free electrons,

implying that the available degree of freedom are purely lattice origin.

The band structure of ScF3 clearly shows a band gap of at least 8 eV which

is an indication of strongly bound valence electrons and empty conduction

band, pernitting classification as an ionic insulator. It should be noted that

ReO3 (introduced in 1.5), a material isostructural to ScF3, happens to be a good

28

metal. The vastly different electronic structures of otherwise similar materials

might be interesting to further investigate.

Since both materials are SNTE materials, it is meaningful to compare the elec-

tronic structures of each with its own distorted structure. Using first principle

calculations, a comparative study [99] has been carried out and the electronic

band structure of distorted ReO3 (O atoms are displaced perpendicular to Re-

O-Re bond) has shown a small destabilization of the flat conduction band

compared with conduction band of non-distorted structure. The atomic dis-

placement was attributed to formation of antibonding orbitals and the authors

conclude that this results in destabilizing the distortion of ReO3 structure. On

the other hand the electronic band structure of distorted ScF3 structure hardly

changes from its non distorted counterpart. Therefore it is concluded that the

ScF3 favors the distortion more than that of ReO3 and as a result the CTE of

ScF3 (αV = -42x10−6/K in 60 K to 110 K temperature window and ∼ -25x10−6/K

at 300 K) is larger than ReO3 (αV = -7.68x10−6/K in 5 K to 300 K temperature

range).

1.8 Motivation

A central question in the study of SNTE is whether basic structural mechanics

principles and intuition can be applied to guide discovery of new materials

that display this anomalous effect. For example, metallic ReO3 and insulating

ScF3 with open perovskite structure display SNTE over a wide range of tem-

29

peratures, but why do other open perovskites most commonly exhibit positive

thermal expansion (PTE)? or can composite materials be formed with thermal

expansion over a wide temperature window, or do stresses inevitably shift the

structural phase to one with PTE? Why is SNTE so rare, inevitably yielding to

PTE in response to disorder and application of pressure?

In pursuit of conceptual control of the phenomenon, innovative approaches

have been offered which link thermally activated transverse vibration of struc-

tural units to a tendency to draw in lattice dimensions. Rigid unit approaches

view polyhedral molecular units (i.e., metal-anion tetrahedra and octahedra)

rather than ions as the fundamental building blocks of a material and attempt

to link the states built from rotational zero modes of the free molecules to the

low-energy modes of the crystal. In this view, intramolecular degrees of free-

dom are effectively integrated out, and the nature of their coordinated motion

as a function of lattice topology and connectivity is the central feature of SNTE.

New discoveries of robust SNTE have reinvigorated the field and raised the

question of whether strict molecular rigidity is an appropriate starting point

or if, instead, it is more appropriate to consider only the rigidity of the stiffest

bonds in a view of the materials as a framework of struts.

30

2.1 Introduction to Inelastic X-ray Scattering

Inelastic x-ray scattering (IXS) is an experimental technique which is used to

investigate distinct forms of material dynamics. In simple words, a collection of

a photon is sent in and the energy and the momentum of the scattered photons

are analyzed which carry information of disparate excitations of the material.

These excitations basically are differentiated by their energies and a schematic

is provided in Figure 2.1.1.

Figure 2.1.1: Excitations that may probe using IXS, From [10]

31

We can identify several distinct methods used in order to probe those excitations

and since there are no sharp boundaries among excitations energies, some of

them may be probed using more than one technique. Table 2.1.1 lists some of

the techniques that fall under the broad interpretation of the IXS.

Technique Incident photon energy

tum density Magnetic Compton 100 keV eV Density of un-

paired spin RIXS(Rasonance) 4-20 keV 0.1 - 50 eV Electron structure

and excitations SIXS(Soft x-ray) 0.1-2 keV 0.01 - 5 eV Electronic and

magnetic struc- ture and excia- tions

NIS(Nuclear IXS) 10-30 keV 1 - 100 meV Element specific phonon and Density of state (DOS)

X-ray Ramam 10 keV 50 - 1000 meV Edge structure, Bonding, Valence

NRIXS 10 keV 0.01 - 10 eV Electronic struc- ture and excita- tion

IXS 10-25 keV 1 - 100 meV Atomic dynamics and phonon dis- persion

Table 2.1.1: List of techniques broadly grouped under the heading of Inelastic X-Ray Scattering.From[10]

2.1.1 IXS advantages over other spectroscopic techniques

One of the significant advantages of IXS is the access to small samples. The

32

synchrotron radiation of high flux and brilliance is capable of focusing the

beam to ∼ 100 microns diameter easily. Even ∼ 10 microns in diameter can

be achieved with some losses. The facts that incoming x-ray photon energy

of ∼ 20 keV is significantly higher than the measured energy transfer of ∼

1-200 meV and the energy and momentum of photon is directly proportional

to each other lead to other compelling advantageous of using IXS such as

decoupling of the energy and momentum transfer, achieving high momentum

resolution and independence of energy resolution from energy transfer. The

Thompson cross section for x-rays is smaller than the absorption scattering

cross section at least by one order of magnitude. This could prevent multiple

scattering from the sample and incoherent scattering at higher energies by only

penetrating into the top 0.01 or 0.1 mm of the sample. Therefore most materials

have very short attenuation length for x-rays which eventually results in lower

background signal as well. But in case of neutron, the scattering cross section

dominates hence multiple scattering can be a problem. On the other hand

higher absorption cross section in x-rays could easily leads to radiation damage

of the material. Nevertheless, it is worthwhile to mention that neutron holds

the edge when higher energy resolution is needed but some of the samples can’t

be measured using neutron scattering or diffraction experiments as they highly

absorb neutrons. Some of the common examples are Cadmium, Samarium and

Europium.

Next section in current chapter is dedicated to elaborate general scattering

33

theory using both classical and quantum mechanical perspectives. It will be

followed by a discussion on probing phonons from a theoretical point of view.

In last section, I will discuss the IXS experimentation to investigate the lattice

dynamics, especially, phonons in crystalline material ScF3.

2.2 Scattering theory

Consider scattering of an x-ray beam from two atoms in an arbitrary lattice

planes of a sample which are separated by distance r. Unlike in x-ray diffraction

the lattice planes can be nonparallel. Lets assume the incoming x-ray wave

vectors are parallel and are denoted by −→ ki . The scattered wave vectors(parallel)

are −→ k f . See Figure 2.2.1 for clear view.

Figure 2.2.1: X-ray scattering from an arbitrary atoms

In order to determine whether the interference is constructive or destructive,

we need to figure out the phase difference between two waves. phase difference

can be obtained by considering the path length difference and can be written

34

as

and using vectors we may write

−→ ki . −→r = |

l1 = λ

Therefore the path length difference can be written as

l = λ

and the phase difference is given by

l 2π λ

−→ Q =

−→ k f − −→ ki (2.2.10)

The scattering wave vector, −→ Q and the spatial arrangement of the atoms in the

sample are key factors when determining the signal at the detector. The spatial

positioning of atom is important since it determines the tendency of sample to

scatter the incoming wave. We can introduce the density of scattering atoms

in the sample to be ρ(−→r ) and assume the scattering density depends on the

36

spatial arrangement of atoms.

Figure 2.2.2: Radiation from source (S) to detector (D) via the sample

Using plane wave approximation and incorporating all above variables, an

expression for the amplitude of the signal at the detector(scattering wave aml-

pitude), fD from a wave emitted by point at tip of the −→r can be written as,

fD ∝ ρ(−→r )ei( −→ ki− −→ k f ).−→r (2.2.11)

fD ∝ ρ(−→r )e−i −→ Q.−→r (2.2.12)

This is specifically derived for one particular point in the sample. Therefore to

calculate the total amplitude at detector we need to integrate over the sample

volume.

37

fD ∝

where V is the total volume of the sample.

Fourier transformation of scattering density leads to the expression

ρ( −→ Q) =

−→ Q.−→r d−→r (2.2.14)

which is similar to the amplitude of the signal at the detector.

To describe the scattering density within one unit cell let us assume the atoms

in the unit cell don’t interact with each other and have their own local scattering

density ρ j( −→ r′ ) where

−→ r′ = −→r − −→r j (2.2.15)

Figure 2.2.3: Reflection geometry where the blue solid circle represents the jth

atom where −→r j and −→r initiate at the unit cell origin

38

ρ j( −→r − −→r j ) (2.2.16)

Now rewriting the total scattering, plugging ρ j( −→ r′ ) and multiplying by 1 =

ei −→ Q.−→r j e−i

−→ Q.−→r j

−→ Q. −→ r′d −→ r′ (2.2.17)

Here the integral term is known as atomic form factor f j( −→ Q) which is a property

of atoms themselves and the summation term ∑

j ei −→ Q.−→r j depends on where the

atoms are located in the lattice. Finally the intensity of scattered beam is given

by

In previous section I have formulated a mathematical expression described

scattering from arbitrary atoms instantaneously at a given time. But we can ex-

tend our analysis further to consider scattering from sample atoms at different

39

times. This of course, results in a phase shift in the scattering wave.

Redefining the scattering density in momentum space and introducing phase

shift e−iωt,

ρ( −→ Q, t) =

Averaging all time to get the total scattering

ρ( −→ Q, ω) =

Writing the intensity of the scattering

S( −→ Q, ω) =

∫ ρ(− −→ Q, t)e−iωtdt (2.2.21)

Shifting t by t + t′

S( −→ Q, ω) =

Performing an average over all time origins

S( −→ Q, ω) =

∫ ρ( −→ Q, 0)ρ(−

40

S( −→ Q, ω) =

−→ Q.−→r k(t)

e−iωtdt (2.2.24)

This is a critical equation in IXS which carries both spatial and time evolution

information about excitations of the system and known as dynamical structure

factor. More importantly for us the signal or the spectra collected in IXS

experiment is directly proportional to dynamic structure factor(S( −→ Q, ω)) of the

material.

Let me start by considering the electron-photon interaction Hamiltonian. Con-

ventionally it can be separated into two terms H0 and Hi, where non interacting

term reads

and electron - photon interaction term is given by

Hi = ∑

j

e2

2mc2

−→p j (2.2.26)

While −→ A and V denotes the electromagnetic field vector and scalar potentials,

41

the electron momentum and position are denoted by−→p and−→r . In Hamiltonian,

Hi the first terms with A2 term dominates in nonresonant scattering processes

while the second term leads in resonant scattering (case where the incoming

energy is tuned into absorption edge of the atom). The nonresonant scattering

cross section depends on dynamic structure factor and has the form of Equation

2.24. Since we only deal with nonresoannt scattering, from here onwards I

would only take H(1) i =

∑ j

e2

2mc2

−→ A2(−→r j ) term into consideration.

Introducing the photon creation (a†kα) and annihilation (akα) operators the vector

potential can be written as

−→ A(−→r ) = L−3/2

−→ k −→r ) (2.2.27)

where ωk, α and k denote the angular frequency, polarization and wave vector

of photon respectively. L3 is normalization box volume.

Let us now consider photon in three dimensional box of side L. The photon

states are quantized and only allowed k values given by 2π/L(nx,ny,nz) where

nx, ny and nz are integers.

Any possible final-state wave-vector k corresponds to a point in wave vector

space with coordinates (kx, ky, kz). Then we can define the density of k states

(number of k points per unit volume) to be L3/(2π)3. In three dimensional

system the k space volume between k′ and k′ + dk′ is 4π2k′2dk′. Therefore the

number of k states in the r